Materials Testing Results - Adhesives and Tapes

Use the links above to access testing results.
==Adhesive and Tapes==
Material Name 	Manufacturer 	Supplier 	Test Results 	Date tested yyyy/mm/dd	Tester 	Test(s) Used 	Description/ Composition 	Comments 	Material Type 	Results Image or Description 	
Scotch-Blue™ 2090 Original Multi-Surface Painter's Tape 	3M 	Consolidated Carpet 	FAIL 	2022/06/17 	MMA 	Oddy Test (method: 20211201_OT ) 	Blue; painter's tape, removable within 12 days, UV and sunlight resistant; 24 mm wide, 54.8 m long roll; contains: polyacrylate 50-55 % by weight; Purchased March 2022 	 	-Polymer - adhesive - single-sided 	 	
2-inch Sigaway® Contact Tape 	Tek Stil Concepts 	Consolidated Carpet 	Temporary 	2022/05/13 	MMA 	Oddy Test (method: 20211201_OT ) 	Brown, nylon fiber reinforced, VOC free acrylic cement film adhesive provided in roll form; contains: acrylic, nylon; Purchased March 2022 	 	-Polymer - adhesive - double-sided 	 	
Tac Tiles™ 	Interface 	Consolidated Carpet 	Temporary 	2022/05/13 	MMA 	Oddy Test (method: 20211201_OT ) 	Clear adhesive squares for installing carpet tiles; PET carrier; 75 x 75 mm square tiles; purchased March 2022 	 	-Polymer - adhesive - single-sided 	 	
DOWSIL™ 3145 RTV silicone, Gray 	Dow 	Dow 	Temporary 	2022/04/29 	MMA 	Oddy Test (method: 20211201_OT ) 	Grey; One-part, moisture RTV, non-flowing, high strength silicone adhesive; contains polydimethysiloxane; Purchased March 2022, cured on aluminum foil for 17 days 	 	-Polymer - adhesive - caulk or sealant 	 	
DOWSIL™ 795 Silicone Building Sealant Black 	Dow 	Dow 	Temporary 	2022/04/29 	MMA 	Oddy Test (method: 20211201_OT ) 	Black; One-part, neutral cure, RTV silicone sealant. Unaffected by sunlight, rain, snow, ozone and temperature extremes of -40°C to 149°C. 3 hr tack free time, 7-14 days of curing time, 14-21 days for full adhesion, 20-30 min. working time, 32 g/L VOC content, 1.52 relative density, contains methanol. Sample purchased March 2022, cured on aluminum foil for 17 days 	 	-Polymer - adhesive - caulk or sealant 	 	
DOWSIL™ 795 Silicone Building Sealant Gray 	Dow 	Dow 	Temporary 	2022/04/29 	MMA 	Oddy Test (method: 20211201_OT ) 	Grey; One-part, neutral cure, RTV silicone sealant. Unaffected by sunlight, rain, snow, ozone and temperature extremes of -40°C to 149°C. 3 hr tack free time, 7-14 days of curing time, 14-21 days for full adhesion, 20-30 min. working time, 32 g/L VOC content, 1.52 relative density, contains methanol and magnesium carbonate. Sample purchased March 2022, cured on aluminum foil for 17 days 	 	-Polymer - adhesive - caulk or sealant 	 	
DOWSIL™ 795 Silicone Building Sealant, Grey 	Dow 	HD Supply 	Temporary 	2022/02/15 	MMA 	Oddy Test (method: 20211201_OT ) 	Grey, neutral, one-part RTV silicone sealant; tack-free in 3 hours, 12 month shelf life; silicone; dispensed onto aluminum foil and cured for 4 days and removed from foil prior to testing; Lot number: H050L39026, purchased: August 2021 	 	-Polymer - adhesive - caulk or sealant 	 	
3M 30-NF Fastbond Contact Adhesive 	3M /solutions.3m.com/en_US/ 	 	pass 	2009/11/13 	NMAI 	Oddy Test 	 	adhesive sandwiched between glass slides, performed better than control, A-D strip test pass 	Adhesive 	Cu: slightly reddish overall, faint black mid coupon; Ag: no change; Pb: no change (except darkening both sides) 	
3M 30-NF Fastbond Contact Adhesive 	3M /solutions.3m.com/en_US/ 	 	pass 	2009/11/13 	NMAI 	Oddy Test 	 	adhesive sandwiched between glass slides, similar to control, A-D strip test pass 	Adhesive 	Cu: reddish, hazy black tarnish at tip from condensation; Ag: no change; Pb: spotty white crystals both sides (sim. To control) 	
3M 30-NF Fastbond Contact Adhesive 	3M /solutions.3m.com/en_US/ 	 	pass 	2009/11/13 	NMAI 	Oddy Test 	 	adhesive on oned side of glass slide, similar to control, A-D strip test pass 	Adhesive 	Cu: reddish, hazy black tarnish at tip from condensation; Ag: no change; Pb: spotty white crystals mostly on side (sim. To control) 	
3M 30-NF Fastbond Contact Adhesive 	3M /solutions.3m.com/en_US/ 	 	pass 	2009/11/13 	NMAI 	Oddy Test 	 	adhesive on oned side of glass slide, performed better than control, A-D strip test pass 	Adhesive 	Cu: reddish, hazy black tarnish at tip from condensation; Ag: no change; Pb: a few white crystals on both sides near tip (condensation) 	
West System 105 Epoxy Resin 	West System, Inc.; www.westsystem.com 	 	pass 	2007/06/14 	NMAI 	Oddy Test 	 	photo on file, A-D strip test pass 	adhesive 	Cu: dull, darkened, interior side irredescent crimson patina; Ag: no change; Pb: dull, darkened 	
West System 105 Epoxy Resin 	West System, Inc.; www.westsystem.com 	 	pass 	2007/06/14 	NMAI 	Oddy Test 	 	sample in jar #8 turned yellow in spots and the top of the cotton plug in water vial also yellowed along edges, A-D strip test pass 	adhesive 	Cu: slightly dull, 2 crimson spots on interior side near fold; Ag: no change; Pb: dull, darkened, slight bluish irredescence 	
3M 1"" Permacel Tape 	3M 	United Manufacturers 	fail 	2007/04/27 	NMAI 	Oddy Test 	 	photo on file 	Adhesive 	Cu: darkened w/ patina; Ag: considerably darkened w/ blue/green patina; Pb: darkened, white powdery surface 	
3M 1"" Permacel Tape 	3M/ 	United Manufacturers 	fail 	2007/04/27 	NMAI 	Oddy Test 	 	photo on file 	Adhesive 	Cu: darkened w/ patina; Ag: considerably darkened w/ blue/green patina; Pb: Darkened 	
Apoxie Sculpt 	Aves www.avesstudio.com 	 	pass 	2007/02/15 	NMAI 	Oddy Test 	 	A-D strip test pass 	adhesive 	Cu: darkened and reddened (same as control); Ag: no change; Pb: no change 	
Apoxie Sculpt 	Aves www.avesstudio.com 	 	pass 	2007/02/15 	NMAI 	Oddy Test 	 	A-D strip test pass 	adhesive 	Cu: darkened and reddened (same as control); Ag: no change; Pb: no change 	
Apoxie Clay - 2 part epoxy putty 	Aves, www.avesstudio.com 	 	pass 	2007/02/08 	NMAI 	Oddy Test 	 	 	adhesive 	Cu: dull, darkened; Ag: no change; Pb: slightly darkened 	
Apoxie Clay - 2 part epoxy putty 	Aves www.avesstudio.com 	 	pass 	2007/02/08 	NMAI 	Oddy Test 	 	 	adhesive 	Cu: dull, darkened; Ag: no change; Pb: slightly darkened 	
3M VHB Adhesive Transfer Tape 9473 PC 	3M Engineered Adhesives Division http://solutions.3m.com/wps/portal/3M/en_US/VHB/Tapes	McMaster-Carr www.mcmaster.com 	pass 	2006/05/11 	NMAI 	Oddy Test 	 	See 3M Scotch VHB Acrylic Foam Double-sided tape #4949 for MSDS 	adhesive 	Cu: dark brown irridescence on half of the coupon; Ag: no change; Pb: darkened; comparable to control 	
3M VHB Adhesive Transfer Tape 9473 PC 	3M Engineered Adhesives Division http://solutions.3m.com/wps/portal/3M/en_US/VHB/Tapes	McMaster-Carr www.mcmaster.com 	pass 	2006/05/11 	NMAI 	Oddy Test 	 	See 3M Scotch VHB Acrylic Foam Double-sided tape #4949 for MSDS 	adhesive 	Cu: comparable to control; Ag: no change; Pb: darkened; comparable to control 	
Double Release Cold-Mount Adhesive DR series DR33100 	Coda, Inc codamount.com 	 	fail 	2006/05/11 	NMAI 	Oddy Test 	 	 	adhesive 	Cu: dark red, dark brown edges; Ag: no change; Pb: thick orange/white buildup on inner side 	
Double Release Cold-Mount Adhesive DR series DR33101 	Coda, Inc codamount.com 	 	fail 	2006/05/11 	NMAI 	Oddy Test 	 	 	adhesive 	Cu: brighter/less red than control; Ag: no change; Pb: darkened; less so than control 	
Epoxy putty ""All Game"" 	Cir-Cut Corporation 4315 North Fourth Street, Phila, PA 19140 (215) 324-1000 	 	fail 	2006/05/11 	NMAI 	Oddy Test 	 	Has been cured in a polyethylene bag for 2 years 	adhesive 	Cu: `; Ag: no change; Pb: dark blue irrisdescence 	
Epoxy putty ""All Game"" 	Cir-Cut Corporation 4315 North Fourth Street, Phila, PA 19140 (215) 324-1000 	 	fail 	2006/05/11 	NMAI 	Oddy Test 	 	Has been cured in a polyethylene bag for 2 years 	adhesive 	Cu: irridescent brown, black edges; Ag: no change; Pb: dark blue irrisdescence 	
Very Hi-bond Acrylic Adhesive Tape 	C.R.Laurence Co., Inc. http://www.crlaurence.com/ 	 	fail 	2006/05/11 	NMAI 	Oddy Test 	 	material remained clear 	adhesive 	Cu: dark brown, black edges; Ag: no change; Pb: darkened; white crystals at inner edge 	
Very Hi-bond Acrylic Adhesive Tape 	C.R.Laurence Co., Inc. http://www.crlaurence.com/ 	 	fail 	2006/05/11 	NMAI 	Oddy Test 	 	material changed from clear to opaque white 	adhesive 	Cu: dark brown, black edges; Ag: no change; Pb: darkened; white crystals at inner edge 	
Nashua 322 Foil tape 	Covalence Adhesives www.covalenceadhesives.com 	 	fail 	2006/05/11 	NMAI 	Oddy Test 	 	 	adhesive/coating 	Cu: comparable to control; Ag: no change; Pb: darkened; comparable to control 	
Nashua 322 Foil tape 	Covalence Adhesives www.covalenceadhesives.com 	 	fail 	2006/05/11 	NMAI 	Oddy Test 	 	possible contamination/interference 	adhesive/coating 	Cu: slight brown irridescence on inner side; Ag: no change; Pb: red-brown crystals on inner side 	
Nashua 322 Foil tape on Appleply 	Covalence Adhesives www.covalenceadhesives.com 	 	fail 	2006/05/11 	NMAI 	Oddy Test 	 	fails as vapor barrier for wood product, A-D strip test: volatile acids produced 	adhesive/coating 	Cu: matte orange; Ag: no change; Pb: thick white crystals overall 	
Nashua 322 Foil tape on Appleply 	Covalence Adhesives www.covalenceadhesives.com 	 	fail 	2006/05/11 	NMAI 	Oddy Test 	 	fails as vapor barrier for wood product, A-D strip test: volatile acids produced 	adhesive/coating 	Cu: brighter/less red than control; Ag: no change; Pb: dusty grey 	
Stik II Polyethylene tape 	Unknown manufacture, used by Guenschel 	 	pass 	2006/03/22 	NMAI 	Oddy Test 	 	 	adhesive 	Cu: no change; Ag: no change; Pb: no change - comparable to control 	
Stik II Polyethylene tape 	Unknown manufacture, used by Guenschel 	 	pass 	2006/03/22 	NMAI 	Oddy Test 	 	 	adhesive 	Cu: no change; Ag: no change; Pb: no change - comparable to control 	
Dow Corning 737 Adhesive 	Dow Corning www.dowcorning.com 	 	pass 	2006/02/25 	NMAI 	Oddy Test 	 	 	adhesive 	Cu: slightly darkened; Ag: no change; Pb: slightly darkened 	
Dow Corning 737 Adhesive 	Dow Corning www.dowcorning.com 	 	pass 	2006/02/24 	NMAI 	Oddy Test 	 	 	adhesive 	Cu: slightly darkened; Ag: no change; Pb: slightly darkened 	
Permacolor Permaprint IP 5000 adhesive in mock graphic panel with 1/8"" acrylic 	MacTac North America www. mactac.com 	 	Pass 	2004/02/09 	NMAI 	Oddy Test 	 	 	Adhesive composite 	Cu: Shiny; Ag: Shiny; Pb: Slightly darkened; violet discolor; slight white corrosion inner & outer ends, condensation? 	
Permacolor Permaprint IP 5000 adhesive in mock graphic panel with 1/8"" acrylic 	MacTac North America www. mactac.com 	 	Pass 	2004/02/09 	NMAI 	Oddy Test 	 	 	Adhesive composite 	Cu: Shiny; Ag: Shiny; Pb: Slightly darkened; bluish discolor - ok 	
Wonderbond WB-104A with WB hardener M-340L 	Borden, Inc., Adhesives & Resins Division www.hexionchem.com 	 	Fail 	2003/12/23 	NMAI 	Oddy Test 	 	Mixed according to instructions & applied to Mylar; curing time 5 days 	adhesive 	Cu: compact tan colored corrosion; mat surfaces; Ag: white hazy effect over most of surface; Pb: fairly even & extensive white corrosion 	
Wonderbond WB-104A with WB hardener M-340L 	Borden, Inc., Adhesives & Resins Division www.hexionchem.com 	 	Fail 	2003/12/23 	NMAI 	Oddy Test 	 	Mixed according to instructions & applied to Mylar; curing time 5 days 	adhesive 	Cu: compact tan colored corrosion; mat surfaces; Ag: white hazy effect over most of surface; Pb: fairly even & extensive white corrosion 	
3M Optically clear adhesive 8141 & 8142 in a mock graphic panel with 1/8"" acrylic, polycarbonate & print media 	3M http://products3.3m.com 	 	Pass 	2003/12/23 	NMAI 	Oddy Test 	 	 	adhesive & graphics composite 	Cu: slight violet tarnishing on inner end; otherwise shiny; Ag: shiny - ok; Pb: slightly dark gray 	
3M Optically clear adhesive 8141 & 8142 in a mock graphic panel with 1/8"" acrylic, polycarbonate & print media 	3M http://products3.3m.com 	 	Pass 	2003/12/23 	NMAI 	Oddy Test 	 	 	adhesive & graphics composite 	Cu: shiny - ok; Ag: shiny - ok; Pb: slightly dark gray 	
Duromount C adhesive in a mock graphic panel with 1/8"" acrylic, polycarbonate & print media 	DuroTech Ahesive Products; www.durotechcorp.com 	 	Pass 	2003/12/23 	NMAI 	Oddy Test 	 	 	adhesive & graphics composite 	Cu: shiny - ok; Ag: shiny - ok; Pb: slightly gray 	
Duromount C adhesive in a mock graphic panel with 1/8"" acrylic, polycarbonate & print media 	DuroTech Ahesive Products; www.durotechcorp.com 	 	Pass 	2003/12/23 	NMAI 	Oddy Test 	 	 	adhesive & graphics composite 	Cu: slight violet tarnishing on inner end; otherwise shiny; Ag: shiny - ok; Pb: slightly gray 	
Lexjet Direct Facemount adhesive in a mock graphic panel with 1/8"" acrylic, polycarbonate & print media 	LexJet Direct www.lexjet.com 	 	Pass 	2003/12/23 	NMAI 	Oddy Test 	 	 	adhesive & graphics composite 	Cu: shiny - ok; Ag: shiny - ok; Pb: slight gray w/blue tinge 	
Lexjet Direct Facemount adhesive in a mock graphic panel with 1/8"" acrylic, polycarbonate & print media 	LexJet Direct www.lexjet.com 	 	Pass 	2003/12/23 	NMAI 	Oddy Test 	 	 	adhesive & graphics composite 	Cu: shiny - ok; Ag: shiny - ok; Pb: slight gray w/blue tinge 	
PermaTrans IP 4000 pressure sensitive adhesive in a mock graphic panel with 1/8"" acrylic, polycarbonate & print media 	MACtac mactac.com 	 	Pass 	2003/12/23 	NMAI 	Oddy Test 	 	 	adhesive & graphics composite 	Cu: shiny - ok; Ag: shiny - ok; Pb: dark gray 	
PermaTrans IP 4000 pressure sensitive adhesive in a mock graphic panel with 1/8"" acrylic, polycarbonate & print media 	MACtac mactac.com 	 	Pass 	2003/12/23 	NMAI 	Oddy Test 	 	 	adhesive & graphics composite 	Cu: shiny - ok; Ag: shiny - ok; Pb: dark gray 	
RemiMount-OC Pressure Sensitive Optically Clear adhesive in a mock graphic panel with 1/8"" acrylic, polycarbonate & print media 	Remington Laminations Inc., www.remingtonlaminations.com 	 	Pass 	2003/12/23 	NMAI 	Oddy Test 	 	 	adhesive & graphics composite 	Cu: shiny - ok; Ag: shiny - ok; Pb: slight gray w/blue/violet tinge 	
RemiMount-OC Pressure Sensitive Optically Clear adhesive in a mock graphic panel with 1/8"" acrylic, polycarbonate & print media 	Remington Laminations Inc., www.remingtonlaminations.com 	 	Pass 	2003/12/23 	NMAI 	Oddy Test 	 	 	adhesive & graphics composite 	Cu: shiny - ok; Ag: shiny - ok; Pb: slight gray w/blue/violet tinge 	
Artsy Decoupage Collage Gel 	Hot Off The Press, Inc.800-227-959-5503-266-9102 	 	Fail 	2003/11/26 	NMAI 	Oddy Test 	 	On Mylar - offgased in fume hood 24+ hrs 	adhesive 	Cu: darkened, beginning to dull; Ag: shiny- ok; Pb: overall even white corrosion 	
Artsy Decoupage Collage Gel 	Hot Off The Press, Inc.800-227-959-5503-266-9102 	 	Fail 	2003/11/26 	NMAI 	Oddy Test 	 	On Mylar - offgased in fume hood 24+ hrs; Corrosion from condensation 	adhesive 	Cu: Shiny. Black corrosion on outer end from condensation; Ag: shiny- ok; Pb: overall even white corrosion 	
Conbond 697 	ITW-TACC www.itwtacc.com 	 	Pass 	2003/11/26 	NMAI 	Oddy Test 	 	Cu coupons for both tested same - seem ok, but discolor of gree/blue unusual - tested on Mylar - offgassed under fume hood for 24+ hrs 	adhesive 	Cu: shiny, slightly darkened, violet & green/blue tinge discolor; Ag: shiny- ok; Pb: dark gray - ok 	
Conbond 697 	ITW-TACC www.itwtacc.com 	 	Pass 	2003/11/26 	NMAI 	Oddy Test 	 	Cu coupons for both tested same - seem ok, but discolor of gree/blue unusual - tested on Mylar - offgassed under fume hood for 24+ hrs 	adhesive 	Cu: shiny, slightly darkened, violet & green/blue tinge discolor; Ag: shiny- ok; Pb: slightly darkened - ok 	
00 NBOND 357 Waterborne Contact Adhesive 	 	 	Pass 	2003/11/10 	NMAI 	Oddy Test 	 	Applied to Mylar & cured for 2 days under fume hood - tested same as Mylar control 	adhesive 	Cu: slightly darkened - still shiny; Ag: shiny - ok; Pb: Slightly darkened - ok 	
00 NBOND 357 Waterborne Contact Adhesive 	 	 	Pass 	2003/11/10 	NMAI 	Oddy Test 	 	Applied to Mylar & cured for 2 days under fume hood - tested same as Mylar control 	adhesive 	Cu: very slightly darkened -stil shiny; Ag: shiny - ok; Pb: Slightly darkened - ok 	
Dry Tac PSF Facemount UV 	 	 	Fail 	2003/11/10 	NMAI 	Oddy Test 	 	 	adhesive 	Cu: darkened and dulled; Ag: shiny - ok; Pb: overall compact white corrosion; green corrosion inside end; reddish corrosion on underside 	
Dry Tac PSF Facemount UV 	 	 	Fail 	2003/11/10 	NMAI 	Oddy Test 	 	 	adhesive 	Cu: darkened and dulled on underside; green on outer end; Ag: shiny - ok; Pb: overall compact white corrosion; reddish corrosion on outer end 	
Drytac Bestmount Flexible BMF adhesive 	 	 	Fail 	2003/11/10 	NMAI 	Oddy Test 	 	 	adhesive 	Cu: shiny - ok; Ag: shiny - ok; Pb: compact even coating of lead carbonate corrosion 	
Drytac Bestmount Flexible BMF adhesive 	 	 	Fail 	2003/11/10 	NMAI 	Oddy Test 	 	 	adhesive 	Cu: violet discoloration, still shiny; Ag: shiny - ok; Pb: compact even coating of lead carbonate corrosion 	
Optimount 60711 	Seal Graphics Americas Corporation www.sealgraphics.com 	 	Fail 	2003/11/10 	NMAI 	Oddy Test 	 	 	adhesive 	Cu: darkened and dulled; Ag: shiny - ok; Pb: compact even coating of lead carbonate corrosion 	
Optimount 60711 	Seal Graphics Americas Corporation www.sealgraphics.com 	 	Fail 	2003/11/10 	NMAI 	Oddy Test 	 	 	adhesive 	Cu: darkened and dulled; Ag: shiny - ok; Pb: compact even coating of lead carbonate corrosion 	
Seal Printmount Plus 60662 Batch # TC1205 Pressure sensitive 	Seal Graphics Americas Corporation www.sealgraphics.com 	 	Fail 	2003/11/10 	NMAI 	Oddy Test 	 	 	adhesive 	Cu: darkened and dulled; Ag: shiny - ok; Pb: compact even coating of lead carbonate corrosion 	
Seal Printmount Plus 60662 Batch # TC1205 Pressure sensitive 	Seal Graphics Americas Corporation www.sealgraphics.com 	 	Fail 	2003/11/10 	NMAI 	Oddy Test 	 	 	adhesive 	Cu: darkened and dulled; Ag: shiny - ok; Pb: compact even coating of lead carbonate corrosion 	
Wilson Art 951 Lockweld Spray Grade Contact Adhesive 	WilsonArt International www.wilsonart.com 	 	Pass 	2003/11/10 	NMAI 	Oddy Test 	 	Applied to Mylar and cured for 2 days under fume hood 	adhesive 	Cu: shiny - ok; Ag: shiny - ok; Pb: Slightly darkened - ok 	
Wilson Art 951 Lockweld Spray Grade Contact Adhesive 	WilsonArt International www.wilsonart.com 	 	Pass 	2003/11/10 	NMAI 	Oddy Test 	 	Applied to Mylar and cured for 2 days under fume hood 	adhesive 	Cu: shiny - ok; Ag: shiny - ok; Pb: Slightly darkened - ok 	
3M VHB adhesive tape 	3M 	 	Fail 	2003/09/15 	NMAI 	Oddy Test 	 	5 week test due to vacation 	adhesive 	Cu: no worse than control # 2: black corrosion on end of coupon outside beaker, rest is shiny ; Ag: shiny - ok; Pb: fairly even white corrosion overall 	
3M VHB adhesive tape 	3M 	 	Fail 	2003/09/15 	NMAI 	Oddy Test 	 	5 week test due to vacation 	adhesive 	Cu: some black corrosion on undreside of coupon; better than control #2; Ag: shiny - ok; Pb: fairly even white corrosion overall 	
Teflon adhesive tape 	 	 	Pass 	2003/09/15 	NMAI 	Oddy Test 	 	5 week test due to vacation 	adhesive 	Cu: shiny - ok; Ag: shiny - ok; Pb: darkened - ok 	
Teflon adhesive tape 	 	 	Pass 	2003/09/15 	NMAI 	Oddy Test 	 	5 week test due to vacation 	adhesive 	Cu: shiny - ok; Ag: shiny - ok; Pb: darkened - ok 	
Viewbond UV 	Quality Mounting & Laminating Systems, Inc. ww.qmis.com 	 	Fail 	2003/08/27 	NMAI 	Oddy Test 	 	Used MSC oven - No Teflon holder used 	Adhesive 	Cu: slight beginnings of black film; slightly dulled; Ag: shiny - ok; Pb: Overall layer white corrosion; some bubbling 	
3M Fastbond contact adhesive (?) on Mylar substrate 	3M 	 	Fail 	2003/08/18 	NMAI 	Oddy Test 	 	Produced bad, irritating smell when jar opened. Adhesive from an unmarked can was used. The can arrived unmarked in Conservation for testing, A-D testing: no change, pH indicator paper: no change 	adhesive 	Cu: Shiny - ok; Ag: Yellow-brown discoloration at bottom; Pb: Slightly darkened - like control 	
3M Fastbond contact adhesive (?) on Mylar substrate 	3M 	 	Fail 	2003/08/18 	NMAI 	Oddy Test 	 	Produced bad, irritating smell when jar opened. Adhesive from an unmarked can was used. The can arrived unmarked in Conservation for testing, A-D testing: no change, pH indicator paper: no change 	adhesive 	Cu: Shiny - ok; Ag: Yellow-brown discoloration overall; Pb: Slightly darkened - like control 	
Viewbond UV 	Quality Mounting & Laminating Systems, Inc. ww.qmis.com 	 	Fail 	2003/07/18 	NMAI 	Oddy Test 	 	Condensation problems for about 1/2 of batch - mainly those nearest the oven door. 	Adhesive 	Cu: Shiny - ok; Ag: shiny - ok; Pb: white corrosion with a yellow tinge 	
Viewbond UV 	Quality Mounting & Laminating Systems, Inc. ww.qmis.com 	 	Fail 	2003/07/18 	NMAI 	Oddy Test 	 	Condensation problems for about 1/2 of batch - mainly those nearest the oven door. 	Adhesive 	Cu: black corrosion bottom, spot of white corrosion - may be condensation; Ag: shiny - ok; Pb: white corrosion overall with yellow crystals 	
# C661 Copper foil tape with non-conductive adhesive 	Saint-Gobain Film Products 800-526-7844 	McMaster-Carr #76555A648 	FAIL 	2003/05/18 	NMAI 	Oddy Test 	 	Possible re test. Suggested by Walter at MSC: copper sulfide produced by large amount of copper foil in test atmosphere may have deposited on Pb coupon then turned to copper metal - could try test with single coupons. 	adhesive 	Cu: Surface darkening & loss of shine ; Ag: shiny; Pb: copper deposits on surface except at edges of coupon 	
# C661 Copper foil tape with non-conductive adhesive 	Saint-Gobain Film Products 800-526-7844 	McMaster-Carr #76555A648 	FAIL 	2003/05/18 	NMAI 	Oddy Test 	 	Possible re test. Suggested by Walter at MSC: copper sulfide produced by large amount of copper foil in test atmosphere may have deposited on Pb coupon then turned to copper metal - could try test with single coupons; less deposition, but also less of sample compared to sample #6	adhesive 	Cu: Surface darkening & loss of shine ; Ag: shiny; Pb: copper deposits on surface except at edges of coupon 	
Jet-Melt 3796 - PG & TC 	3M www.3m.com 	 	PASS 	2003/05/16 	NMAI 	Oddy Test 	 	Condensation problems.Left in oven 1 week longer than normal for T of 60 C 	adhesive 	Cu: Mostly shiny, slight haze, darkened slightly, dark spot from condensation; Ag: shiny; Pb: darkened 	
Jet-Melt 3796 - PG & TC 	3M www.3m.com 	 	PASS 	2003/05/16 	NMAI 	Oddy Test 	 	Condensation problems.Left in oven 1 week longer than normal for T of 60 C 	adhesive 	Cu: Mostly shiny, slight haze, darkened slightly, black corrosion on bottom corner - condensation prob; Ag: shiny; Pb: darkened - lead carbonate on bottom corner - condensation prob 	
Fastbond Contact Adhesive 2000 -NF 	3M3M www.3m.com 	 	Pass 	2003/04/22 	NMAI 	Oddy Test 	 	No control used 	adhesive 	Cu: slightly discolored; Ag: shiny; Pb: darkened 	
Fastbond Contact Adhesive 2000 -NF 	3M3M www.3m.com 	 	Pass 	2003/04/22 	NMAI 	Oddy Test 	 	No control used 	adhesive 	Cu: slightly discolored; Ag: Shiny; Pb: darkened 	
Permatrans IP 2100 adhesive 	MACtac North America www.mactac.com 	 	Fail 	2003/04/22 	NMAI 	Oddy Test 	 	No control used 	adhesive 	Cu: darkened, violet, dulled surface; Ag: shiny; Pb: darkened, violet color 	
Permatrans IP 2100 adhesive 	MACtac North America www.mactac.com 	 	Fail 	2003/04/22 	NMAI 	Oddy Test 	 	No control used 	adhesive 	Cu: violet color, black corrosion bottom, ; Ag: shiny; Pb: white corrosion very bubbly, condensation 	
Tyvek Tape #4711 	Dupont 	Masterpak 	Temporary 	2021/09/22 	MMA 	Oddy Test (method: 20190226_OT_1 ) 	Item Number 1-907; Tear resistant nonwoven polyethylene with a corona treatment adhesive tape, made with Dupont's Tyvek Number 1075D; acid-free acrylic adhesive; 1 inches x 36 yards; Purchased August 2021 	 	-Polymer - adhesive - single-sided 	 	
Feather-rite autobody filler 	US Chemical 	Unknown 	Fail 	2021/09/10 	MMA 	Oddy Test (method: 20190226_OT_1 ) 	Blue; 2-part tack-free and lightweight autobody filler; 757 mL pail and 21.2 g hardener, 3-5 minute setting time at room temperature; 9.8 g filler and 0.2 g hardener mixed together and spread in a thin layer on mylar to cure for 5 days before testing; Purchased June 2021 	 	-Paste - filler/binder mixtures (eg.: plaster, spackle) 	 	
3M 425 Aluminum Foil Tape, 15D114 	3M 	Grainger 	Temporary 	2021/08/19 	MMA 	Oddy Test (method: 20190226_OT_1 ) 	Single sided pressure sensitive tape with a metallic carrier; 1 inch wide, 4.6 mils thick; adhesion to steel: 51 N/100 mm; thermally conductive, chemical and moisture resistant, acrylic adhesive; Purchased May 2021 	 	-Polymer - adhesive - single-sided 	 	
Heat n' Bond Lite 	Therm O Webb 	Amazon 	Temporary 	2021/08/19 	MMA 	Oddy Test (method: 20190226_OT_1 ) 	Clear and permanent double-sided iron-on adhesive on a paper backing; 43 cm by 4.8 m; To apply, remove paper backing and adhere on medium heat pressing iron down for 6 seconds on each section; Purchased May 2021, sample heated with an iron between sheets of mylar prior to testing 	 	-Polymer - adhesive - glue - heat activated 	 	
Pellon 805 Wonder-Under® Iron-on adhesive 	Pellon 	Amazon 	Temporary 	2021/08/19 	MMA 	Oddy Test (method: 20190226_OT_1 ) 	Iron-on fusible adhesive on pellon; acid-free 100% polyester; 38.1 cm by 1.8 m; Purchased May 2021, sample heated with an iron between sheets of mylar prior to testing 	 	-Polymer - adhesive - glue - heat activated 	 	
Lascaux Acrylic Adhesive 303HV 	Lascaux Colours and Restauro 	Talas 	Temporary 	2021/08/12 	MMA 	Oddy Test (method: 20191213_B_OT ) 	Extremely elastic liquid adhesive that dries tacky; thermoplastic copolymer butyl-methacrylate dispersion thickened with acrylic butyl-ester, pH 8-9 biocide stabilized; Catalog number TAD018004; Purchased February 2020 	 	-Polymer - adhesive - glue - liquid 	 	
Evacon R Copolymer Emulsion 	Conservation By Design 	Conservation Resources 	Fail 	2021/08/12 	MMA 	Oddy Test (method: 20191213_B_OT ) 	White; Reversible paper laminating adhesive (EVA); water soluble, non-plasticized pH 7.5, ethylene-vinyl acetate copolymer emulsion, contains <0.1% formaldehyde; Catalog number EVAR-1; Purchased May 2021 	 	-Polymer - adhesive - glue - liquid 	 	
Lascaux Acrylic Adhesive 498 HV 	Lascaux Colours and Restauro 	Talas 	Temporary 	2021/08/12 	MMA 	Oddy Test (method: 20191213_B_OT ) 	Elastic liquid adhesive that dries hard; thermoplastic acrylic resin composed of a water-based emulsion containing butylacrylate thickened with methacrylic acid (40% solids); Catalog number TAD019004; Purchased February 2020 	 	-Polymer - adhesive - glue - liquid 	 	
Quick Cure 5 epoxy 	Bob Smith Industries 	Bob Smith Industries 	Temporary 	2021/07/28 	MMA 	Oddy Test (method: 20190226_OT_1 ) 	2-part 5 minute cure epoxy, permanent; will harden in 5 minutes at room temperature with slight flexibility, 1 hour full cure; Contains: bisphenol A epoxy resin, poly-mercaptan hardener; mixed together 10mL of Part A and 10mL of Part B and spread on mylar to cure for 2 days prior to testing; Purchased May 2021 	 	-Polymer - adhesive - glue - liquid 	 	
S-700 Floor Tile Adhesive 	Armstrong Flooring 	Consolidated Carpet 	Fail 	2021/06/10 	MMA 	Oddy Test (method: 20190226_OT_1 ) 	Black VCT floor tile adhesive; water-based rosin and asphalt rubber; 18 hour working time; moisture and alkali resistant, nonflammable, ammonia-free, low odor; manufactured September 2020, purchased April 2021, spread in a thin layer on mylar and cured for 6 days before testing 	 	-Polymer - adhesive - glue - liquid 	 	
S-515 floor tile adhesive 	Armstrong Flooring 	Consolidated Carpet 	Temporary 	2021/06/10 	MMA 	Oddy Test (method: 20190226_OT_1 ) 	VCT floor tile adhesive; water-based latex resin; 24 hour working time; moisture and alkali resistant; manufactured March 2021, purchased April 2021, spread in a thin layer on mylar and cured for 6 days before testing 	 	-Polymer - adhesive - glue - liquid 	 	
S-799 Adhesive 	Armstrong Flooring 	RoundSquare/Beyer Blinder Belle 	Fail 	2021/06/10 	MMA 	Oddy Test (method: 20190226_OT_1 ) 	High moisture adhesive for PVC-free sheet and rubber tile; 25 minute working time; contains glass and oxides; spread on mylar and cured for 6 days before testing; Purchased April 2021 	 	-Polymer - adhesive - glue - liquid 	 	
Quilters Select(TM) Appli-Web Pus, #QSAWP-1X10 	RNK Distributing 	Red Rock Threads, Inc 	Temporary 	2021/06/01 	MMA 	Oddy Test (method: 20190226_OT_1 ) 	Light-weight and flexible, permanent fusible adhesive webbing; 1-inch wide roll; Polyurethane ester aliphatic; purchased December 2019; sample ironed between mylar and removed from mylar before testing 	 	-Polymer - adhesive - glue - heat activated 	 	
BBT(r) Bio-flooring Adhesive, S-525 	Armstrong 	Consolidated Carpet 	Temporary 	2021/05/14 	MMA 	Oddy Test (method: ) 	Water-based latex liquid floor tile adhesive; 20 minute open time, 24 hour working time; 16 g/L VOC; 2 year shelf life; Purchased 2021, cured in a thin layer on mylar for 9 days prior to testing, mylar in the jar 	 	-Polymer - adhesive - glue - liquid 	 	
635 Book Tape, 31-0141 	The Library Store 	The Library Store 	Temporary 	2021/05/06 	MMA 	Oddy Test (method: 20190226_OT_1 ) 	Clear, acid-free tape; 2 inches wide, 3.5-mil gloss polypropylene, acrylic adhesive; Purchased February 2021 	 	-Polymer - adhesive - pressure-sensitive 	 	
J-Lar II(r), Heavy-Duty Book Repair Tape 	Unknown 	The Library Store 	Fail 	2021/04/29 	MMA 	Oddy Test (method: 20190226_OT_1 ) 	Single-sided, pressure sensitive, acid-free tape; 2 inches wide, 3.5 mil gloss polypropylene, 60lb tensile strength; Purchased February 2021 	 	-Polymer - adhesive - single-sided 	 	
Biodegradable Cello Carton Sealing Tape 	Unknown 	Ecoenclose 	Fail 	2021/04/29 	MMA 	Oddy Test (method: 20190226_OT_1 ) 	Single-sided, pressure sensitive tape with a plant-derived cellulose backing and renewable and biodegradable rubber adhesive; compostable around 100 degrees F, ASTM D6400; 2 inches wide; contains rubber and hydrocarbon resin adhesive derived from conifers; Purchased March 2021 	 	-Polymer - adhesive - single-sided 	 	
Magic Smooth 	Wesco Enterprises 	ArtPlace 	Fail 	2021/04/13 	MMA 	Oddy Test (method: 20190226_OT_1 ) 	2-part epoxy that doesn't dissolve foams; sets firmly overnight; Mixed 1:1 by volume resin and hardener and spread on mylar with a glass slide, cured for 6 days; purchased January 2019 	 	-Polymer - adhesive - glue - liquid 	 	
FIBERseal 	Ductmate 	Unknown 	Temporary 	2021/04/13 	MMA 	Oddy Test (method: 20190226_OT_1 ) 	1 gallon bucket of fiber reinforced duct sealant used to seal metal joints against air leaks in high pressure duct systems up to 15" W.G.; synthetic latex, fiber, water; should be cured for 24-72 hours for before pressure testing; material spread on mylar with a glass slide and cured for 6 days; purchased February 2021 	 	-Polymer - adhesive - caulk or sealant 	 	
METHOCEL™ A4C Methylcellulose 	Dow 	Dow 	PASS 	2021/03/19 	MMA 	Oddy Test (method: 20190226_OT_1 ) 	Water-soluble, high purity, non-ionic cellulose ether that performs as thickener, binder, and film former. Also functions as a suspending aid, stabilizer, surfactants, lubricants, protective colloids, and emulsifiers. Consists of methylcellulose, water, and sodium chloride. Received February 2020, tested in solid form. Not dissolved or prepared in any way prior to testing 	 	Polymer - adhesive - glue - liquid 	 	
DOWSIL™ 795 Silicone Building Sealant White 	Dow Corning 	Amazon 	Temporary 	2021/03/19 	MMA 	Oddy Test (method: 20190226_OT_1 ) 	One-part, neutral cure, RTV silicone sealant, unaffected by sunlight, rain, snow, ozone and temperature extremes of -40°C to 149°C. 3 hr tack free time, 7-14 days of curing time, 14-21 days for full adhesion, 20-30 min. working time, 32 g/L VOC content, 1.52 relative density, contains methanol and diisopropoxydi(ethoxyacetoacetyl)titanate. Purchased January 2020, cured for 24 days 	 	Polymer - adhesive - caulk or sealant 	 	
Dowsil 791 Silicone Weatherproofing Sealant 	Dow Corning 	Dow 	Temporary 	2021/03/19 	MMA 	Oddy Test (method: 20190226_OT_1 ) 	One-part, neutral-cure, grey RTV silicone sealant; 20 minute working time, 40 minute tack-free time, 7-14 days to cure; 31 g/L VOC, 1.46 relative density; Contains dodecamethylcyclohexasiloxane and unsaturated fatty acids treated with calcium carbonate; Purchased February 2020; applied to mylar and spread into an even layer about 2 mm thick using a glass slide, cured for 15 days 	 	Polymer - adhesive - caulk or sealant 	 	
3M™ Sprayable Hot Melt Adhesive 6111 	3M 	3M 	Temporary 	2021/03/19 	MMA 	Oddy Test (method: 20190226_OT_1 ) 	100% solids, sprayable polyolefin copolymer thermoplastic adhesive. 0.92 g/mL density, 177-196°C application temperature, 1 min open time surface foam to PVC, 6 min open time surface foam to foam. Contains hydrocarbon resin, polyolefin copolymer, and polypropylene. Sheet of Mylar placed on hot plate at 185°C, rubbed glue stick against it in circles to melt and cure; cured for 15 days 	 	Polymer - adhesive - glue - heat activated 	 	
Titebond III Ultimate Wood Glue 	Franklin International 	Amazon 	FAIL 	2021/02/18 	MMA 	Oddy Test (method: 20190226_OT_1 ) 	One-part, waterproof wood glue, proprietary polymer-based formula. 1.11 relative density, 98.889°C boiling point. Purchased March 2020, applied to mylar and spread out thinly using a glass slide, cured for 2 days. 	 	Polymer - adhesive - glue - liquid 	 	
VHB 4952 Acrylic foam tape 	3M 	3M 	Temporary 	2020/12/02 	MMA 	Oddy Test (method: 20190226_OT_1 ) 	White, low surface energy, high strength permanent bond adhesive with a firm acrylic foam core; 2 cm width, 0.045 (1.1mm) thick; 24 month shelf life; lot number 19324; Purchased October 2020 	 	Polymer - adhesive - double-sided 	 	
Filmoplast P90 	Neschen 	Talas 	Temporary 	2020/12/02 	MMA 	Oddy Test (method: 20190226_OT_1 ) 	Self adhesive white archival paper tape; 50 g/m^2; acid-free, buffered with calcium carbonate, age-resistant permanent acrylic adhesive, non-yellowing, solvent-free; Purchased 	 	Polymer - adhesive - single-sided 	 	
P.C. Woody epoxy, Part A and B 	Protective Coating Company 	Protective Coating Company 	Temporary 	2020/12/02 	MMA 	Oddy Test (method: 20190226_OT_1 ) 	Two part bulked epoxy filler; Part A contains Bisphenol A - Epichlorohydrin polymer, Kaolin, Hydrous magnesium silicate, Bis(2-ethylhexyl) terephthalate, Glycidyl Ethers of Bisphenol F Resin, Titanium Dioxide, Polyethylene fiber. Part B contains Styrenated phenol, Kaolin, Aliphatic Polyaminoamide, Polyoxypropylenediamine, Talc, N-Aminoethyl piperazine, Bis(2-ethylhexyl) terephthalate; workable for 1/2 hour, 12-24 hour full cure; Prepared in a 1:1 mixture by weight and applied to mylar with a wooden tongue depressor, cured 2 days prior to testing, removed from mylar before testing; Purchased March 2020 	 	Paste - filler/binder mixtures (eg.: plaster, spackle) 	 	
Lineco Frame Sealing Tape Gray, L387-0151 	Lineco, Holyoke 	Lineco 	PASS 	2020/11/12 	MMA 	Oddy Test (method: 20190226_OT_1 ) 	Manufactured from Perma/Seal label stock with a foil layer, a non-yellowing, permanent acrylic adhesive. Acid-free, lignin-free, with aluminum barrier. Sample purchased August 2020 	 	Polymer - adhesive - single-sided 	 	
3M™ Scotchcal™ Luster Overlaminate 3645 	3M 	3M 	FAIL 	2020/10/22 	MMA 	Oddy Test (method: 20190226_OT_1 ) 	Slip-resistant overlaminate designed for floor graphics; 7.874 mil thick; printable vinyl and pressure-sensitive acrylic adhesive; Received September 2020 	 	Polymer - adhesive - single-sided 	 	
Aquazol 500 	Polymer Chemistry Innovations] 	Talas 	Temporary 	2020/10/22 	MMA 	Oddy Test (method: 20190226_OT_1 ) 	Poly(2-ethyl-2-oxazoline), also known as PEOX or PEtOx, is a non-toxic, non-hazardous, and biocompatible water-soluble polymer. Kinematic viscosity range of 18-24 cSt, refractive index of 1.52, glass temperature of 69°C, neutral pH. Off-white solid Purchased February 2020, tested in solid form. Not dissolved or prepared in anyway prior to testing 	 	Polymer - adhesive - glue - liquid 	 	
Klucel G 	Hercules/Ashland 	Talas 	Temporary 	2020/10/22 	MMA 	Oddy Test (method: 20190226_OT_1 ) 	Non-ionic adhesive (hydroxypropylcellulose) soluble in water and alcohol, mixes well with hot waxes. Thermoplastic, dries clear and very flexible. Often used as a leather consolidant and as an adhesive with vellums. Insoluble at temperatures above 113°F (45 C), pH value of 5-8.5 in water solution, softening point of 212-302°F (100-150 C). Purchased February 2020, tested as a dry powder without dissolving or additional preparation 	 	Polymer - adhesive - glue - liquid 	 	
Double Coated Urethane Foam Tape, 4056 	3M 	3M 	FAIL 	2020/10/16 	MMA 	Oddy Test (method: 20190226_OT_1 ) 	Black double sided foam tape with green and white liner; 1.6 mm thick; polyurethane foam and pressure-sensitive acrylic adhesive; liner removed before testing 	 	Polymer - adhesive - double-sided 	 	
ITac Plus Vinyl Laminate 	Continental Grafix 	Continental Grafix 	FAIL 	2020/10/16 	MMA 	Oddy Test (method: 20190226_OT_1 ) 	White vinyl laminate with pressure sensitive adhesive. PVC and unknown adhesive. Coated paper backing removed for Oddy test. Received 3/2019 	 	Polymer - adhesive - pressure-sensitive 	 	
Crompton Heat-Set Tissue 	Crompton 	Talas 	Temporary 	2020/10/21 	MMA 	Oddy Test (method: 20190226_OT_1 ) 	Long fibered heat activated abaca hemp tissue coated on one side with an acrylic archival heat set adhesive (Texicryl/Paraloid). 9g/m^2, pH netural, reversible with mineral spirits. Prepared by heating to 176-197F between mylar sheets, tested without mylar. Purchased January 2020 	 	Polymer- adhesive - glue - heat activated 	 	
Filmoplast R 	Neschen 	Talas 	Temporary 	2020/10/21 	MMA 	Oddy Test (method: 20190226_OT_1 ) 	Light, transparent, technical Japanese paper, coated with heat actiavted acrylic-acid ester copolymer. Free of lignin and hemicellulose, with a high percentage of alpha cellulose. Adhesive is colorless, ageing-resistant, free of softeners, contains magnesium carbonate, and does not yellow. 8.5 g/m^2, sealing temperature must be over 100°C. Purchased January 2020 	 	Polymer - adhesive - glue - heat activated 	 	
Fusion 4000 Dry Mount Adhesive 	D&K 	D&K 	FAIL 	2020/10/21 	MMA 	Oddy Test (method: 20190226_OT_1 ) 	Ultra-clear, removable, thermal activated, 100% inert, acid-free pure adhesive film. Recommended temperature of 175°F. Sample cut from a roll produced within the past year. Activated on hot plate between two sheets of Mylar at 80°C, pressed down firmly by a beaker, peeled from Mylar. Received January 2020, cured 12 days 	 	Polymer - adhesive - glue - heat activated 	 	
BEVA 371 Film 	Conservator's Products Company 	Conservator's Products Company 	FAIL 	2020/10/21 	MMA 	Oddy Test (method: 20190226_OT_1 ) 	Made of pure BEVA 371 solution, sandwiched between two sheets: one of 1.5-mil silicone-coated Mylar release film and a sheet of 4-mil silicone-coated release paper. Solvent-free. Activated on hot plate between two sheets of Mylar at 65°C, pressed down firmly by a beaker, adhesive layer peeled from Mylar and the original backing. Received January 2020, cured 12 days 	 	Polymer - adhesive - glue - heat activated 	 	
Hot_melt_glue_stick_comparison#Product_Tabless 3M™ Hot Melt Adhesive 3779Q 	3M 	3M 	Temporary 	2020/10/21 	MMA 	Oddy Test (method: 20190226_OT_1 ) 	100% solids hot melt adhesive. 0.99 g/mL density, 177-196°C application temperature, 25 sec open time, 75 sec delivery time. Contains polyamide polymer. Sheet of Mylar placed on hot plate at 180°C, rubbed glue stick against it in circles to melt and cure. Received September 2020, cured 12 days 	 	Polymer - adhesive - glue - heat activated 	 	
Hot_melt_glue_stick_comparison#Product_Tables 3M™ Hot Melt Adhesive 3797TC 	3M 	Digi-Key 	Temporary 	2020/10/21 	MMA 	Oddy Test (method: 20190226_OT_1 ) 	100% solids hot melt adhesive. 0.92 g/mL density, 177-196°C application temperature, 30 sec open time, 55 sec delivery time. Contains polypropylene, hydrocarbon resin, polyethylene, ethylene-propylene copolymer, antioxidant, and polyolefin wax. Sheet of Mylar placed on hot plate at 180°C, rubbed glue stick against it in circles to melt and cure. Purchased September 2020, cured 12 days 	 	Polymer - adhesive - glue - heat activated 	 	
Hot_melt_glue_stick_comparison#Product_Tables 3M™ Hot Melt Adhesive 3748Q 	3M 	Arrow 	PASS 	2020/10/21 	MMA 	Oddy Test (method: 20190226_OT_1 ) 	100% solids, no VOCs thermoplastic resin. 0.93 g/mL density, 177-196°C application temperature, 45 sec open time, 65 sec delivery time. Contains polypropylene, hydrocarbon resin, styrene-butadiene polymer, ethylene-propylene polymer, polyethylene, and non-hazardous additives. Sheet of Mylar placed on hot plate at 180°C, rubbed glue stick against it in circles to melt and cure. Purchased September 2020, cured 12 days 	 	Polymer - adhesive - glue - heat activated 	 	
Lascaux 498 HV 	Lascaux 	Talas 	Temporary 	2020/10/08 	MMA 	Oddy Test (method: 20190226_OT_1 ) 	Thermoplastic acrylic resin composed of a water-based dispersion butyl acrylate and methylmethacrylate thickened with acrylic butylester. Water thinnable, insoluble in water when dry. Permanently soluble in acetonem toluene, xylene, etc. Min film formation temp of ~5°C, glass transition temperature of ~6°C, 400% elongation at break, minimum sealing temperature of ~68-76°C, elastic hard dry film consistency. 100°C boiling point, 1.0 g/cm3 density. Purchased November 2018, opened April 2019, cured for 7 days 	 	Polymer - adhesive - glue - liquid 	 	
Wheat Starch Aytex-P 	ADM Arkady 	Talas 	Temporary 	2020/10/08 	MMA 	Oddy Test (method: 20190226_OT_1 ) 	Highly refined, unmodified food grade wheat starch. Used in bookbinding and paper conservation as an adhesive for paper, leather, fabric, and other porous materials. High water holding capacity, pH 5-6.5 (measured in 70% slurry). To buffer, add 10% (by weight) of calcium carbonate. Bulk density of 32 lb/ft^3 (512.6 kg/m^3) loose, 45 lb/ft^3 (720.8 kg/m^3) packed. Purchased February 2020, cured for 7 days 	 	Polymer - adhesive - glue - liquid 	 	
Lineco Frame Sealing Tape White, L387-0152 	Lineco, Holyoke 	Lineco 	Temporary 	2020/10/08 	MMA 	Oddy Test (method: 20190226_OT_1 ) 	Manufactured from Perma/Seal label stock with a foil layer, a non-yellowing, permanent acrylic adhesive. Acid-free, lignin-free, with aluminum barrier. Purchased August 2020 	 	Polymer - adhesive - single-sided 	 	
GE Supreme Silicone 	General Electric Company 	Lowe's 	FAIL 	2020/10/08 	MMA 	Oddy Test (method: 20190226_OT_1 ) 	100% silicone and waterproof sealant that provides a reliable seal in weather-prone areas like windows, doors, basements, roofs, sidewalks, siding, tuckpointing and attics. Contains octamethylcyclotetrasiloxane, hexamethyldisilazane, and dibutyl tin bis acetylacetonate. Purchased August 2020, cured for 7 days 	 	Polymer - adhesive - caulk or sealant 	 	
GE Silicone II Clear Caulk #GE5000 	General Electric Company 	Amazon 	FAIL 	2020/10/08 	MMA 	Oddy Test (method: 20190226_OT_1 ) 	Waterproof one-part silicone sealant. 28 g/L VOC, 5-10 min work life, 20-30 min tack-free time, 2-3 day cure time, temperature range of -55°F to 400°F, relative density of 1.006. Contains hydrotreated middle distillates (petroleum), hexamethyldisilazane, and dibutyl tin bis acetylacetonate. Purchased August 2020, cured for 7 days 	 	Polymer - adhesive - caulk or sealant 	 	
XT-765, 2-part silicone 	Silicone Inc. 	Silicones Inc. 	FAIL 	2020/09/29 	MMA 	Oddy Test (method: 20190226_OT_1 ) 	Thixotropic tin catalyzed RTV-2 silicone. 40 min work time, 6 month shelf life, 1.10 specific gravity. 0.99 relative density for part A, 1.10 relative density for part B. Part A contains polydimethyl siloxane, silicon dioxide, trimethoxyphenylsilane, tetrapropyl orthosilicate, dimethyltin dineodecanoate, and green pigment. Part B contains polydimethylsiloxane, silicon dioxide, titanium diooxide, and trihydroxystearin. Received March 2020, cured for 5 days 	 	Polymer - adhesive - caulk or sealant 	 	
XP-565, 2-part silicone 	Silicone Inc. 	Silicones Inc. 	FAIL 	2020/09/29 	MMA 	Oddy Test (method: 20190226_OT_1 ) 	Transparent, two-component, addition reaction, platinum catalyzed silicone rubber. Designed to remain water-clear even after extended exposure to the sun. 1.5 hr work time, 1.02 specific gravity, -60 to 600°F service temperature. 0.98 relative density for part A, 1.02 relative density for part B. Part A contains polydimethylsiloxane dimethylvinyl terminated and dimethyl, methylhydrogen polydimethylsiloxane. Part B contains platinum catalyst and polydimethylsiloxane, dimethylvinyl terminated. Received March 2020, cured for 5 days 	 	Polymer - adhesive - caulk or sealant 	 	
XT-493, 2-part silicone 	Silicone Inc. 	Silicones Inc. 	FAIL 	2020/09/29 	MMA 	Oddy Test (method: 20190226_OT_1 ) 	Thixotropic, two-component, tin catalyzed RTV silicone rubber. Designed for casting polyurethanem polyester and epoxy parts. 1.10 specific gravity, 1-1.5 hr working time, 6 month shelf life. 0.99 relative density for part A, 1.10 relative density for part B. Part A contains dibutyltin dilaurate, ethyl silicate, polymeric ethyl silicate, silicon dioxide, blue pigment, and polydimethyl siloxane. Part B contains polydimethylsiloxane, silicon dioxide, titanium dioxide, and trihydroxystearin. Received March 2020, cured for 5 days 	 	Polymer - adhesive - caulk or sealant 	 	
GI 1000, 2-part silicone 	Silicone Inc. 	Silicones Inc. 	FAIL 	2020/09/29 	MMA 	Oddy Test (method: 20190226_OT_1 ) 	Two-part tin-catalyzed RTV-2 silicone rubber designed for casting polyester parts. 1.5-2.5 hr working time, 6 month shelf life, -60 to 350°F service temperature, 1.09 specific gravity. 0.99 relative density for part A, 1.1 relative density for part B. Part A contains dibutyltin dilaurate, ethyl silicate, polymeric ethyl silicate, silicon dioxide, blue pigment, and polydimethyl siloxane. Part B contains polydimethylsiloxane, silicon dioxide, and titanium dioxide. Received March 2020, cured for 5 days 	 	Polymer - adhesive - caulk or sealant 	 	
3M™ Scotch-Weld™ Epoxy Adhesive 420 Off-White 	3M 	3M 	Temporary 	2020/09/29 	MMA 	Oddy Test (method: 20190226_OT_1 ) 	Two-part epoxy, part A contains modified epoxy resin, 4,7,10-Trioxatridecane-1,13-Diamine, 2,4,6-tris((Dimethylamino)Methyl)Phenol, amorphous silica, and calcium salt, and part B contains epoxy resin and acrylic polymer. Sample received August 2020, cured for 5 days. 	 	Polymer - adhesive - glue - liquid 	 	
Fibre Glast 2000 Epoxy Resin + Fibre Glast 2060 Epoxy Hardener 	Fibre Glast 	Fibre Glast 	FAIL 	2020/09/29 	MMA 	Oddy Test (method: 20190226_OT_1 ) 	Two-part epoxy, resin contains epoxy resin based mixture and multifunctional acrylate, and hardener contains modified amine mixture. Purchased in 2017, cured for 5 days. 	 	Polymer - adhesive - glue - liquid 	 	
West System G/Flex 650 Toughened Epoxy 	Gougeon Brothers, Inc 	Amazon 	FAIL 	2020/09/29 	MMA 	Oddy Test (method: 20190226_OT_1 ) 	Two-part Epoxy resin and Rubber modified-polyamine mixture. Part A: Propane, 2,2-bis[p-(2,3-epoxypropoxy)phenyl], polymers, Phenol-Formaldehyde Polymer Glycidyl Ether. Part B: ATBN polymer, Non-hazardous, Triethylenetetramine, Benzene-1,3-dimethanamine, Phenol, 2,4,6-tris[(dimethylamino)methyl] reaction products with triethylenetetramine, Tris-2, 4, 6(dimethylaminomethyl) phenol, Aminoethylpiperazine, Tetraethylenepentamine. Purchased March 2020, cured for 5 days 	 	Polymer - adhesive - glue - liquid 	 	
West System 105 Epoxy Resin® / 205 Fast Hardener® 	Gougeon Brothers, Inc 	Gougeon Brothers, Inc 	FAIL 	2020/09/29 	MMA 	Oddy Test (method: 20190226_OT_1 ) 	Two-part epoxy used for general coating and bonding applications at lower temperatures. 1.18 specific gravity, 1-4 days for cure. 105 contains benzyl alcohol, phenol-formaldehyde polymer glycidyl ether, and propane, 2,2-bis[p-(2,3-epoxypropoxy)phenyl]-, polymers. 205 contains hydroxybenzene, tetraethylenepentamine, triethylenetetramine, polyethylenepolyamines, reaction products of triethylenetetramine with phenol and formaldehyde, and triethylenetetramine, reaction products with propylene oxide. Received February 2020, cured for 5 days 	 	Polymer - adhesive - glue - liquid 	 	
Araldite® AW 4859 / Hardener HW 4859 	Huntsman 	Huntsman 	Temporary 	2020/09/29 	MMA 	Oddy Test (method: 20190226_OT_1 ) 	Two-component, epoxy adhesive paste of high strength and toughness. AW 4859 (1.2 specific gravity) contains 2,2'-[(1-methylethylidene)bis(4,1-phenyleneoxymethylene)]bisoxirane, 4,4'-isopropylidenebis[2-allylphenol], and glass, oxide, chemicals. Hardener HW 4859 (specific gravity of 1.0) contains 4,7,10-trioxatridecane-1,13-diamine, 4-methylcyclohexane-1,3-diamine, 2-methylcyclohexane-1,3-diamine, 2-piperazin-1-ylethylamine, and 2-Propenenitrile, polymer with 1,3-butadiene, 1-cyano-1-methyl-4-oxo-4-[[2-(1-piperazinyl)ethyl]amino]butyl-terminated. Received July 2020, cured for 5 days 	 	Polymer - adhesive - glue - liquid 	 	
Titebond III Ultimate Wood Glue 	Franklin International 	Amazon 	FAIL 	2020/09/25 	MMA 	Oddy Test (method: 20190226_OT_1 ) 	One-part, waterproof wood glue, proprietary polymer-based formula. Non-toxic, solvent free. 98.889°C boiling point. 24 month shelf life. 20-25 minute total assembly time; Purchased March 2020, cured for 1 day 	 	Polymer - adhesive - glue - liquid 	 	
3M™ Hi-Strength 90 CA Spray Adhesive - Low VOC <25% 	3M 	iTapeStore 	FAIL 	2020/09/25 	MMA 	Oddy Test (method: 20190226_OT_1 ) 	A clear, industrial grade high strength aerosol spray adhesive. 0.863 g/mL density, <25% VOC, 1-4 min dry time, synthetic elastomer base. Contains methyl acetate, dimethyl ether, propane, 1,1-difluoroethane, hexmethyldisiloxane, cyclohexane, chlorobenzotrifluoride, and N-butyl acetate. Purchased July 2020, cured for 1 day 	 	Polymer - adhesive - glue - liquid 	 	
3M™ Foam Fast 74 CA Spray Adhesive - Low VOC <25% 	3M 	Amazon 	FAIL 	2020/09/25 	MMA 	Oddy Test (method: 20190226_OT_1 ) 	A clear, industrial grade high strength lace spray adhesive. 0.853 g/mL density, <25% VOC, 30s-2 min dry time, synthetic elastomer base. Contains methyl acetate, dimethyl ether, propane, 1,1-difluoroethane, hexmethyldisiloxane, cyclohexane, chlorobenzotrifluoride, and N-butyl acetate. Purchased July 2020, cured for 1 day 	 	Polymer - adhesive - glue - liquid 	 	
3M™ Super 77™ CA Multi-Purpose Spray Adhesive - Low VOC <25% 	3M 	Amazon 	FAIL 	2020/09/25 	MMA 	Oddy Test (method: 20190226_OT_1 ) 	A translucent, high tack and fast drying mist spray adhesive. 0.80 g/mL density, <25% VOC, 15-30s dry time, synthetic elastomer base. Contains acetone, 1,1-difluoroethane, propane, and cyclohexane. Purchased July 2020, cured for 1 day 	 	Polymer - adhesive - glue - liquid 	 	
RTV615, 2-part silicone 	GE Silicones 	Momentive 	FAIL 	2020/09/18 	MMA 	Oddy Test (method: 20190226_OT_1 ) 	Silicone rubber compound, clear liquid that cures at room temperature to high strength silicone rubber with the addition of curing agents. Parts A and B mixed 10:1 by weight, specific gravity of 1.02 for part A, temperature range of -60 to 204°C, 4 hr. work time, 6-7 day full cure. Contains octamethylcyclotetrasiloxane. Received January 2020, cured for 13 days 	 	Polymer - adhesive - caulk or sealant 	 	
LiquidWood Epoxy Wood Consolidant 	Abatron 	Ace Hardware 	FAIL 	2020/09/18 	MMA 	Oddy Test (method: 20190226_OT_1 ) 	Two-part epoxy wood consolidant consisting of a resin and a hardener, mix parts A and B 1:1 by volume. Part A contains bisphenol-a-(epichlorhydrin), 2,3-epoxypropyl o-tolyl ether, butyl glycidyl ether, and γ-butyrolactone. Part B contains tetraethylene pentamine and fatty acids, tall-oil, reaction products with tetraethylenepentamine. Cured for 13 days. Purchased February 2020 	 	Polymer - adhesive - glue - liquid 	 	
Lok Lift Adhesive Netting 	Optitech 	Optitech 	Temporary 	2020/09/08 	MMA 	Oddy Test (method: 20190226_OT_1 ) 	Coarse adhesive netting with yellow backing, adhesive for flooring installation of surfaces including wood, carpet, vinyl, etc; adhered to thin Mylar for Oddy testing. Received July 2020 	 	Polymer - adhesive - double-sided 	 	
Fusible Bonding Web for Medium Fabrics, 261 	Dritz 	Amazon 	FAIL 	2020/09/08 	MMA 	Oddy Test (method: 20190226_OT_1 ) 	Fusible bonding web for medium fabrics, UPC:072879280258, for use with steam iron; 18 x 36 inches; 100% polyamide; Purchased December 2019, sample material ironed between sheets of mylar before testing 	 	Polymer - adhesive - glue - heat activated 	 	
Heritage Gummed Paper Tape #TAD101002 	Klug Conservation 	Talas 	Temporary 	2020/04/03 	MMA 	Oddy Test (method: 20190226_OT_1 ) 	Single-sided paper tape with gumming; 2.5 cm width roll; components: potato starch, paper; Received June 2019 	 	Polymer - adhesive - single-sided 	 	
Dowsil 3145 Silicone Adhesive Clear MIL-A-46146, 4812MKTW 	Dow Corning 	Ellsworth Adhesive, Inc. 	Temporary 	2020/04/03 	MMA 	Oddy Test (method: 20190226_OT_1 ) 	Neutral cure silicone adhesive; 90mL tube; date of manufacture: March 1, 2019 - Lot No. H050J31072; Prepared 1/27/2020, extruded through the 1/2" nozzle opening in lines onto aluminum foil. After setting for four days, cut into ~1cm lengths. Pieces mixed on aluminum foil by hand (wearing nitrile gloves). Purchased December 2019 	 	Polymer - adhesive - glue - liquid 	 	
Hot-melt_glue_stick_comparison#Product_Tables Hot Melt Adhesive 3764Q 	3M 	McMaster-Carr 	FAIL 	2020/04/03 	MMA 	Oddy Test (method: 20190226_OT_1 ) 	Low temp hot-melt glue for 3M EC and TC guns; catalog number 7333A37; ethylene-vinyl acetate polymer, naphtha, hydrocarbon resin; solid stick 5/8" x 8"; Prepared on 7/2/2019 and 7/5/2019; Extruded with a used 3M Plygun LT with Quadrack Converter (no temperature settings). Remains of previous glue stick and first new glue stick extruded and discarded. Extruded in dots onto aluminum foil. Dots mixed in large glass lab beaker by hand (wearing nitrile gloves). Purchased May 2019 	 	Polymer - adhesive - glue - heat activated 	 	
Scotch-Weld Urethane Adhesive DP605NS 	3M 	3M 	FAIL 	2020/03/27 	MMA 	Oddy Test (method: 20190226_OT_1) 	Two-part, 1:1 mix ratio, non-sagging, semi-flexible, thixotropic urethane adhesive. Boiling point of 178°C, density of 1.17 g/mL, glass transition temperature of 41°C. Contains diphenylmethane diisocyanate, polymethylene polyphenyl isocyanate, polypropylene glycols, and amorphous silica. Sample received February 2020, cured for 1 week prior to testing 	Color: Off-white 	Polymer - adhesive - glue - liquid 	 	
Scotch-Weld Epoxy Adhesive DP100 	3M 	3M 	Temporary 	2020/03/27 	MMA 	Oddy Test (method: 20190226_OT_1) 	Two-part, 1:1 mix ratio, fast-curing rigid epoxy adhesive containing mercaptan polymer, tris(2,4,6-Dimethylaminomonomethyl)phenol, bis((Dimethylamino)methyl)phenol, and Poly(Bisphenol A-co-epichlorohydrin). Color may vary from nearly white to yellow/amber. Boiling points of parts A and B are 93°C and 260°C and densities are 1.13 g/mL and 1.17 g/mL respectively. Glass transition temperature of 33°C. Sample received February 2020, cured for 1 week prior to testing 	Color: Yellow, amber 	Polymer - adhesive - glue - liquid 	 	
Gorilla Heavy Duty Construction Adhesive 	The Gorilla Glue Company 	Amazon 	Temporary 	2020/03/27 	MMA 	Oddy Test (method: 20190226_OT_1) 	Waterproof construction adhesive with application temperature of 40 to 100°F and service temperature of -40 to 200°F. Consists of limestone, calcium carbonate, stearic acid, quartz, and dibutyltin bis(acetylacetonate). Sample received February 2020, cured for 1 week prior to testing 	Color: White 	Polymer - adhesive - caulk or sealant 	 	
Jade 711 PVA Adhesive 	Unknown 	Talas 	FAIL 	2020/03/25 	MMA 	Oddy Test (method: 20190226_OT_1) 	Acid-free polyvinyl acetate adhesive similar to Jade 403, with reduced odor. For use on paper, fabric, board, canvas, leather, and film. 1.05-1.10 g/cm3 density, pH 7.1-7.3, initial boiling point of >212°F. Sample received January 2020, cured for 5 days prior to testing 	Color: White 	Polymer - adhesive - glue - liquid 	 	
Jade R Reversible PVA Bookbinding Adhesive 	Unknown 	Talas 	FAIL 	2020/03/25 	MMA 	Oddy Test (method: 20190226_OT_1) 	Acid-free multi polymer (PVA and EVA) water reversible adhesive. For use on paper, board, leather and fabric. 1.05-1.10 g/cm3 density, pH 7.1-7.3, initial boiling point of >212°F. Sample received January 2020, cured for 5 days prior to testing 	Color: White 	Polymer - adhesive - glue - liquid 	 	
White Gorilla Glue 	The Gorilla Glue Company 	Amazon 	Temporary 	2020/03/25 	MMA 	Oddy Test (method: 20190226_OT_1) 	100% waterproof white polyurethane glue. Bonds to foam, wood, metal, ceramic, and stone. Contains 4,4’diphenylmethane diisocyanate, 2,4’diphenylmethane diisocyanate, and Oxirane, methyl, polymer with .alpha.hydro.omega.-hydroxypolyoxy(methyl-1,2-ethanediyl) and 1,1-methylenebisisocyanatobenzene. Sample received February 2020, cured for 5 days prior to testing 	Color: White 	Polymer - adhesive - glue - liquid 	 	
Titebond II Premium Wood Glue 	Franklin International 	Franklin International 	FAIL 	2020/03/25 	MMA 	Oddy Test (method: 20190226_OT_1) 	Cross-linking polyvinyl acetate wood glue with strong initial tack and fast to set. 3.0 g/L VOC, relative density of 1.09, pH 3.0. Honey cream colored as liquid, translucent/yellow as dried film. Contains aluminum chloride. Sample received February 2020, cured for 5 days prior to testing 	Color: Yellow 	Polymer - adhesive - glue - liquid 	 	
Titebond Original Wood Glue 	Franklin International 	Franklin International 	FAIL 	2020/03/25 	MMA 	Oddy Test (method: 20190226_OT_1) 	Aliphatic resin emulsion wood glue with strong initial tack and fast to set. 10.7 g/L VOC, relative density of 1.0771, pH 4.0. Yellow as liquid, translucent as dried film. Sample received February 2020, cured for 5 days prior to testing 	Color: Yellow 	Polymer - adhesive - glue - liquid 	 	
Sikaflex®-11 FC Sealant Adhesive 	Sika 	HD Supply 	FAIL 	2020/03/25 	MMA 	Oddy Test (method: 20190226_OT_1) 	One part polyurethane, moisture-cured elastomeric sealant/adhesive. For use on cement, ceramics, glass, metals, wood, and epoxy. Service temperature of -40°F to 170°F, 1-2 hour tack-free time, 3-5 day final cure time. Contains xylene, 4,4'-methylenediphenyl diisocyanate, ethylbenzene, and silica quartz. Sample purchased January 2020, cured for 12 days prior to testing 	Color: White 	Polymer - adhesive - caulk or sealant 	 	
SilGlaze* II Silicone Sealant, SCS2800 	GE Silicones 	Amazon 	FAIL 	2020/03/25 	MMA 	Oddy Test (method: 20190226_OT_1) 	One-part, neutral, fast cure, medium modulus silicone sealant, primerless adhesion. 33 g/L VOC, density of 1.035 g/cm3, 6-12 min work life, 30 min tack free time, 24 hour cure time, 3-4 days for full cure, temperature range of -55°F to 300°F. Contains octamethylcyclotetrasiloxane, hexamethyldisilazane, and dibutyl tin bis acetylacetonate. Sample purchased January 2020, cured for 12 days prior to testing 	Color: Clear 	Polymer - adhesive - caulk or sealant 	 	
DOWSIL™ 795 Silicone Building Sealant Gray 	Dow Corning 	Amazon 	FAIL 	2020/03/25 	MMA 	Oddy Test (method: 20190226_OT_1) 	One-part, neutral cure, RTV silicone sealant. Unaffected by sunlight, rain, snow, ozone and temperature extremes of -40°C to 149°C. 3 hr tack free time, 7-14 days of curing time, 14-21 days for full adhesion, 20-30 min. working time, 32 g/L VOC content, 1.52 relative density, contains methanol and magnesium carbonate. Sample purchased January 2020, cured for 14 days prior to testing 	Color: Gray 	Polymer - adhesive - caulk or sealant 	 	
DOWSIL™ 795 Silicone Building Sealant Black 	Dow Corning 	Amazon 	FAIL 	2020/03/25 	MMA 	Oddy Test (method: 20190226_OT_1) 	One-part, neutral cure, RTV silicone sealant. Unaffected by sunlight, rain, snow, ozone and temperature extremes of -40°C to 149°C. 3 hr tack free time, 7-14 days of curing time, 14-21 days for full adhesion, 20-30 min. working time, 32 g/L VOC content, 1.52 relative density, contains methanol. Sample purchased January 2020, cured for 14 days prior to testing 	Color: Black 	Polymer - adhesive - caulk or sealant 	 	
3M Rubber and Vinyl 80 Spray Adhesive 	3M 	3M 	FAIL 	2020/03/19 	MMA 	Oddy Test (method: 20190226_OT_1) 	A high performance polychloroprene based contact aerosol spray adhesive. 0.835g/mL density, 12.9% solids content by weight, <55% VOC, 3 min dry time, 3 - 30 min bonding range. Contains methyl acetate, dimethyl ether, cyclohexane, toluene, naphthol spirits, rosin, and zinc oxide. Sample received February 2020, cured for 1 day prior to testing 	Color: Yellow 	Polymer - adhesive - glue - liquid 	 	
Hi-Strength 90 Spray Adhesive 	3M 	3M 	FAIL 	2020/03/19 	MMA 	Oddy Test (method: 20190226_OT_1) 	An industrial grade synthetic elastomer spray adhesive that is typically used for bonding HPL to wood. 0.69g/mL density, 13% solids content by weight, <55% VOC, 1 min dry time, 1 - 10 min bonding range. Contains dimethyl ether, isobutane, acetone, pentane, cyclohexane, and propane. Sample received February 2020, cured for 1 day prior to testing 	Color: Clear 	Polymer - adhesive - glue - liquid 	 	
Foam Fast 74 Spray Adhesive 	3M 	3M 	FAIL 	2020/03/19 	MMA 	Oddy Test (method: 20190226_OT_1) 	An extremely fast tacking industrial grade synthetic elastomer spray adhesive for bonding foam and fabric. 0.718 g/mL density, 22% solids content by weight, <55% VOC, 30s dry time, 30 sec - 15 min bonding range. Contains dimethyl ether, isobutane, acetone, pentane, methyl acetate, cyclohexane, petroleum naphtha, cyclopentane, and drometrizole (antioxidant, an aromatic conjugated amine). Sample received February 2020, cured for 1 day prior to testing 	Color: Clear 	Polymer - adhesive - glue - liquid 	 	
Briteline Shield, UV Matte Overlaminate 	Grimco 	Grimco 	FAIL 	2020/03/05 	MMA 	Oddy Test (method: 20190226_OT_1) 	Calendered PVC matte overlaminate; permanent acrylic adhesive; protection against UV degradation, moisture, and abrasion; 1 year shelf life; 3 mil thickness; Purchased December 2019 	Color: Green 	Polymer - adhesive - single-sided 	 	
3M 4952 Very High Bond (VHB) Tape 	3M 	McMaster-Carr 	Temporary 	2018/01/04 	FMNH 	Oddy Test 	White acrylic foam with rubber adhesive on Kraft paper liner, double-sided, 3/4" 	 	Polymer - adhesive tape - double sided 	--Copper: Consistent with Control
--Lead: Overall gray haze and white crystal growth on edges
--Silver: Consistent with Control 	
3M 465 Adhesive Tape 	3M 	Grainger 	Pass, Permanent 	2018/01/16 	FMNH 	Oddy Test 	Clear, double-sided acrylic transfer tape 	 	Polymer - adhesive tape - double sided 	--Copper: Consistent with Control
--Lead: Consistent with Control
--Silver: Consistent with Control 	
3M Double-Coated Medical Tape 	3M 	 	Pass, Permanent 	2018/03/30 	FMNH 	Oddy Test 	Double-sided sheet adhesive on transparent polyethylene film 	 	Polymer - adhesive tape - double sided 	--Copper: Consistent with Control
--Lead: Consistent with Control
--Silver: Consistent with Control 	
Glue Dots, Permanent 	Glue Dots International , LLC 	Office Max 	Pass, Permanent 	2018/03/30 	FMNH 	Oddy Test 	Double-sided adhesive. Translucent oval with a blue tinge. Comes in different oval sizes. 	 	Polymer - adhesive - pressure-sensitive 	--Copper: Consistent with Control
--Lead: Consistent with Control
--Silver: Consistent with Control 	
Very High Bond Acrylic-Adhesive Tape 	C.R. Laurence Company, Inc. 	C.R. Laurence Company, Inc. 	Fail, Unsuitable 	2018/06/04 	FMNH 	Oddy Test 	Double-sided clear tape - 1/4" w. 	 	Polymer - adhesive tape - double sided 	--Copper: Hazy with red to black color change
--Lead: Minor white crystal accumulation
--Silver: Consistent with Control 	
Glue Dots, Removable 	Glue Dots International , LLC 	Office Max 	Pass, Permanent 	2017/10/24 	FMNH 	Oddy Test 	Double-sided. Removable, clear, comes in different diameters or ovals. 	 	Polymer - adhesive - pressure-sensitive 	--Copper: Consistent with Control
--Lead: Orange haze consistent with control
--Silver: Consistent with Control 	
MacTac Adhesive - MAC IP5000 Perma Print RL Mounting Adhesive 	Mactac 	Agfa Corporation 	Fail, Unsuitable 	2017/10/24 	FMNH 	Oddy Test 	Double-sided, acrylic, pressure-sensitive film 	 	Polymer - adhesive - pressure-sensitive 	--Copper: Red discoloration
--Lead: Consistent with Control
--Silver: Black discoloration 	
FEP Teflon tape with Silicone Adhesive 	 	CS Hyde Co. 	Pass, Permanent 	2016/06/14 	FMNH 	Oddy Test 	Optically-clear, pressure-sensitive PTFE tape 	 	Polymer - adhesive tape - single sided 	--Copper: Consistent with Control
--Lead: Consistent with Control
--Silver: Consistent with Control 	
3M ATG #9082 	3M 	 	Fail, Unsuitable 	2006/02/21 	BKM 	Oddy Test 	acid free adhesive transfer (double sided, no carrier) 	 	Polymer - adhesive tape - double sided 	Pb: 3/21/06: fail, green and white with areas of orange/red. Also, overall very small platelets of shiny white/iridescent. This was not on control; 
Cu: 3/21/06: fail, dark black corrosion at both tips, more than control; 
Ag: 3/21/06: pass 	
3M Aluminum Foil Tape #431 	3M 	 	Temporary 	2006/02/23 	BKM 	Oddy Test 	2"" wide, acrylic adhesive 	Pass for short term exhibition, not long term 	Polymer - adhesive tape - single sided 	Pb: 3/23/06: pass, intermediate (light green on inside edge, slight white on outside edge); 
Cu: 3/23/06: pass (very slight iridescence at tip of coupon); 
Ag: 3/23/06: pass 	
3M scotch #853 	3M 	 	Fail, Unsuitable 	2006/02/23 	BKM 	Oddy Test 	polyester film with acrylic adhesive 	 	Polymer - adhesive tape - single sided 	Pb: 3/23/06: fail (orange/red at inside tip grown along side very light white along tip); 
Cu: 3/23/06: pass; 
Ag: 3/23/06: pass 	
Nashua #330X 	Nashua 	 	Pass, Permanent 	2006/04/04 	BKM 	Oddy Test 	Aluminum foil tape with pressure sensitive acrylic adhesive 	 	Polymer - adhesive tape - single sided 	Pb: 4/28/06: unspecified temp: pass; 
Cu: 4/28/06: unspecified temp: pass, very slight overall darkening, same as control; 
Ag: 4/28/06: pass 	
3M Scotch-Weld Epoxy Adhesive Tube Kit 2212 	3M 	 	Pass, Permanent 	2007/02/14 	BKM 	Oddy Test 	B/A grey 	No specific results for metals or temps. Comments ""great- no tarnish pass"" 	Paste - filler/binder mixture (non-paint) 	Pb: ; 
Cu: ; 
Ag: 	
3M VHB 9473 adhesive transfer tape 	3M 	 	Pass, Permanent 	2008/12/30 	BKM 	Oddy Test 	 	 	Polymer - adhesive tape - double sided 	Pb: no date: no change; 
Cu: no date: no change; 
Ag: no date: no change 	
Gudy 808 	Neschen 	 	Pass, Permanent 	2008/12/30 	BKM 	Oddy Test 	permanent water based acrylic adhesive 	 	Polymer - adhesive 	Pb: no date: no change; 
Cu: no date: no change; 
Ag: no date: no change 	
Adchem 254-74 Tape 	Adchem 	 	Pass, Permanent 	2009/02/10 	BKM 	Oddy Test 	double faced acrylic pressure sensitive adhesive tape with release liner 	same result as Volara sample, but slightly more corroded than control 	Polymer - adhesive tape - double sided 	Pb: 3/10/09: very slightly corroded; 
Cu: 3/10/09: very slightly corroded; 
Ag: 3/10/09: ok 	
3M hot melt glue #3792 	3M 	 	Pass, Permanent 	2009/03/16 	BKM 	Oddy Test 	 	pass but should not be used in direct contact with object or in sealed case 	Polymer - adhesive 	Pb: 4/13/09: appearance of brownish yellow material on surface; 
Cu: 4/13/09: tarnished slightly; 
Ag: 	
3M hot melt glue #3797 	3M 	 	Pass, Permanent 	2009/03/16 	BKM 	Oddy Test 	 	pass but should not be used in direct contact with object or in sealed case 	Polymer - adhesive 	Pb: 4/13/09: appearance of brownish yellow material on surface; 
Cu: 4/13/09: tarnished slightly; 
Ag: 	
3M 415 double sided tape "splicing tape" 	3M 	Talas 	Pass, Permanent 	2016/07/05 	BKM 	Oddy Test 	uses 3M adhesive 400 (medium firm acrylic pressure sensitive adhesive system), carrier is a polyester film, liner is tan #60 kraft paper 	 	Polymer - adhesive tape - double sided 	Pb: no change; 
Cu: very slight darkening, no significant corrosion; 
Ag: no change 	
3M 465 double sided tape 	3M 	Talas 	Pass, Permanent 	2016/07/05 	BKM 	Oddy Test 	uses 3M adhesive 400 (medium firm acrylic pressure sensitive adhesive system), no carrier film, liner is tan #60 kraft paper 	 	Polymer - adhesive tape - double sided 	Pb: no change; 
Cu: very slight darkening, no significant corrosion; 
Ag: no change 	
3M VHB / Acrylic Foam Tape 4910 F 	3M 	 	Pass, Permanent 	2016/08/04 	BKM 	Oddy Test 	Acrylic foam tape 	Cu corrosion appeared the same as on both controls 	Polymer - adhesive tape - double sided 	Pb: No corrosion; 
Cu: minor darkening; 
Ag: no corrosion 	
Dow Corning 3145 RTV MIL-A-46146 Transparent / Structural Sealant and Adhesive 	Dow Corning 	 	Pass, Permanent 	2017/05/26 	BKM 	Oddy Test 	Silicone adhesive 	same as controls 	Polymer - adhesive caulk 	Pb: dark gray, same as control; 
Cu: red - same as control; 
Ag: no corrosion 	
Dow Corning RTV Sealant 737 Neutral Cure Sealant 	Dow Corning 	 	Fail, Unsuitable 	2017/05/26 	BKM 	Oddy Test 	Silicone adhesive 	much more corrosion on Pb than control 	Polymer - adhesive caulk 	Pb: white corrosion, none on control; 
Cu: red - same as control; 
Ag: no corrosion 	
3M Scotch 924 ATG tape, clear 	3M 	 	Pass, Permanent 	2017/05/26 	BKM 	Oddy Test 	Adhesive 400 (medium firm acrylic, pressure sensitive), no carrier film 	same as controls 	Polymer - adhesive tape - single sided 	Pb: dark gray, same as control; 
Cu: red - same as control; 
Ag: no corrosion 	
3M Bumpon 	3M 	 	Fail, Unsuitable 	2017/05/26 	BKM 	Oddy Test 	Polyurethane acrylic-adhesive backed pads (Resilient rollstock-clear series, SJ5600) 	different from control, a better alternative to this product was already found 	Polymer - sheet (>1mm thick) 	Pb: some white corrosion, none on control; 
Cu: 1 coupon purplish, other very red, both darker than control; 
Ag: no corrosion 	
3M Scotch Blue Tape 2090 	3M 	Amazon 	Pass, Permanent 	2017/06/23 	BKM 	Oddy Test 	Acrylic-adhesive backed washi paper (low-medium adhesion) 	Only 1 out of 2 sample jars were able to be opened, yet both looked okay 	Polymer - adhesive tape - single sided 	Pb: No corrosion; 
Cu: no corrosion; 
Ag: no corrosion 	
3M Scotch Blue Tape 2080 	3M 	Amazon 	Pass, Permanent 	2017/06/23 	BKM 	Oddy Test 	Acrylic-adhesive backed crepe paper, (medium adhesion) 	 	Polymer - adhesive tape - single sided 	Pb: no corrosion; 
Cu: no corrosion; 
Ag: no corrosion 	
J-Lar Super Clear Tape (Shurtape) 	J-Lar 	 	Pass, Permanent 	2018/11/27 	BKM 	Oddy Test 	clear tape 	 	Polymer - adhesive tape - single sided 	Pb: very slight yellowing, similar to control; 
Cu: darkened slightly (purple-red) same as control; 
Ag: same as control 	
Versimold rubber compound 	Rowe Industries 	 	Pass, Permanent 	2018/12/17 	BKM 	Oddy Test 	rubber compound 	 	Polymer - block/bulk/pellet 	Pb: no corrosion; 
Cu: darkened slightly compared to control; 
Ag: no corrosion 	
Sugru Mouldable Glue, Original Formula, Black, semi-cured 	Sugru 	 	Fail, Unsuitable 	2019/01/25 	BKM 	Oddy Test 	mouldable glue 	semi-cured (~6 hours) Control lead FAIL 	Polymer - block/bulk/pellet 	Pb: Control lead FAIL; 
Cu: rainbow corrosion from edges; 
Ag: same as control 	
Sugru Mouldable Glue, Original Formula, Black, semi-curedSugru Mouldable Glue, Original Formula, White, semi-cured 	Sugru 	 	Fail, Unsuitable 	2019/01/25 	BKM 	Oddy Test 	mouldable glue 	semi-cured (~6 hours) Control lead FAIL 	Polymer - block/bulk/pellet 	Pb: Control lead FAIL; 
Cu: overall yellowed compared to control; 
Ag: same as control 	
Sugru Mouldable Glue, Original Formula, Black, fully cured 	Sugru 	 	Fail, Unsuitable 	2019/01/31 	BKM 	Oddy Test 	mouldable glue 	fully cured - re-test with longer set/cure time 	Polymer - block/bulk/pellet 	Pb: yellowish corrosion; 
Cu: overall yellowed compared to control; 
Ag: same as control 	
Sugru Mouldable Glue, Original Formula, White, fully cured 	Sugru 	 	Fail, Unsuitable 	2019/01/31 	BKM 	Oddy Test 	mouldable glue 	fully cured - re-test with longer set/cure time 	Polymer - block/bulk/pellet 	Pb: yellowish corrosion; 
Cu: overall yellowed compared to control; 
Ag: same as control 	
Kraftmark Pro-Create Professional Sculptors Putty 	Kraftmark 	 	Pass, Permanent 	2008/12/30 	BKM 	Oddy Test 	2 part epoxy putty 	Ok to useif allowed to cure for two weeks. Better to use outside case. 	Paste - filler/binder mixture (non-paint) 	Pb: ; 
Cu: Date Unknown: corroded; 
Ag: 	
Kraftmark Pro-Create Professional Sculptors Putty 	Kraftmark 	 	Pass, Permanent 	2008/12/30 	BKM 	Oddy Test 	2 part epoxy putty (white and grey), similar to pliacre, 60hr air time, 50/50 mix ratio 	Pass if allowed to cure for 2+ weeks. Oddy tested 5/8/08, new Oddy test requested 	Paste - filler/binder mixture (non-paint) 	Pb: ; 
Cu: ; 
Ag: 	
Magic Sculpt 2 part epoxy putty 	Wesco 	 	Pass, Permanent 	2009/03/27 	BKM 	Oddy Test 	cured for two weeks 	considered for use in mountmaking 	Paste - filler/binder mixture (non-paint) 	Pb: ; 
Cu: 4/17/09: oxidized; 
Ag: 	
Magic Sculpt White 	Wesco 	 	Pass, Permanent 	2009/03/27 	BKM 	Oddy Test 	2 part epoxy putty cured 2 weeks 	considered for use in mountmaking 	Paste - filler/binder mixture (non-paint) 	Pb: ; 
Cu: 4/17/09: oxidized; 
Ag: 	
Pro-Create Terrain Putty (2 part) 	Kraftmark 	 	Pass, Permanent 	2009/03/27 	BKM 	Oddy Test 	2 part epoxy putty cured 2 weeks 	considered for use in mountmaking 	Paste - filler/binder mixture (non-paint) 	Pb: ; 
Cu: 4/17/09: oxidized; 
Ag: 	
Promante MC Bond 2K Transparent / Structural Adhesive 	Promanté 	 	Pass, Permanent 	2016/09/21 	BKM 	Oddy Test 	Structural adhesive 	Cu corrosion appeared the same as on both controls 	Polymer - adhesive caulk 	Pb: No corrosion; 
Cu: minor darkening; 
Ag: no corrosion 	
3M ATG #9082 	3M 	 	Fail, Unsuitable 	2006/02/21 	BKM 	Oddy Test 	acid free adhesive transfer (double sided, no carrier) 	 	Polymer - adhesive tape - double sided 	Pb: 3/21/06: fail, green and white with areas of orange/red. Also, overall very small platelets of shiny white/irridescent. This was not on control; 
Cu: 3/21/06: fail, dark black corrosion at both tips, more than control; 
Ag: 3/21/06: pass 	
3M VHB 9473 adhesive transfer tape 	3M 	 	Pass, Permanent 	2008/12/30 	BKM 	Oddy Test 	 	 	Polymer - adhesive tape - double sided 	Pb: no date: no change; 
Cu: no date: no change; 
Ag: no date: no change 	
Adchem 254-74 Tape 	Adchem 	 	Pass, Permanent 	2009/02/10 	BKM 	Oddy Test 	double faced acrylic pressure sensitive adhesive tape with release liner 	same result as Volara sample, but slightly more corroded than control 	Polymer - adhesive tape - double sided 	Pb: 3/10/09: very slightly corroded; 
Cu: 3/10/09: very slightly corroded; 
Ag: 3/10/09: ok 	
3M 415 double sided tape "splicing tape" 	3M 	Talas 	Pass, Permanent 	2016/07/05 	BKM 	Oddy Test 	uses 3M adhesive 400 (medium firm acrylic pressure sensitive adhesive system), carrier is a polyester film, liner is tan #60 kraft paper 	 	Polymer - adhesive tape - double sided 	Pb: no change; 
Cu: very slight darkening, no significant corrosion; 
Ag: no change 	
3M 465 double sided tape 	3M 	Talas 	Pass, Permanent 	2016/07/05 	BKM 	Oddy Test 	uses 3M adhesive 400 (medium firm acrylic pressure sensitive adhesive system), no carrier film, liner is tan #60 kraft paper 	 	Polymer - adhesive tape - double sided 	Pb: no change; 
Cu: very slight darkening, no significant corrosion; 
Ag: no change 	
3M VHB / Acrylic Foam Tape 4910 F 	3M 	 	Pass, Permanent 	2016/08/04 	BKM 	Oddy Test 	Acrylic foam tape 	Cu corrosion appeared the same as on both controls 	Polymer - adhesive tape - double sided 	Pb: No corrosion; 
Cu: minor darkening; 
Ag: no corrosion 	
3M Aluminum Foil Tape #431 	3M 	 	Temporary 	2006/02/23 	BKM 	Oddy Test 	2"" wide, acrylic adhesive 	Pass for short term exhibition, not long term 	Polymer - adhesive tape - single sided 	Pb: 3/23/06: pass, intermediate (light green on inside edge, slight white on outside edge); 
Cu: 3/23/06: pass (very slight irridescence at tip of coupon); 
Ag: 3/23/06: pass 	
3M scotch #853 	3M 	 	Fail, Unsuitable 	2006/02/23 	BKM 	Oddy Test 	polyester film with acrylic adhesive 	 	Polymer - adhesive tape - single sided 	Pb: 3/23/06: fail (orange/red at inside tip grown along side very light white along tip); 
Cu: 3/23/06: pass; 
Ag: 3/23/06: pass 	
Nashua #330X 	Nashua 	 	Pass, Permanent 	2006/04/04 	BKM 	Oddy Test 	Aluminum foil tape with pressure sensitive acrylic adhesive 	 	Polymer - adhesive tape - single sided 	Pb: 4/28/06: unspecified temp: pass; 
Cu: 4/28/06: unspecified temp: pass, very slight overall darkening, same as control; 
Ag: 4/28/06: pass 	
3/8"" Linen Tape 	Talas 	Talas 	Pass, Permanent 	2019/09/18 	BKM 	Oddy Test 	70% linen 30% cotton; unbleached and unsized 	 	Polymer - adhesive tape - single sided 	Pb: same as control; 
Cu: same as control; 
Ag: same as control 	
3M Super 77 Multipurpose Spray Adhesive 	3M 	Amazon 	Temporary 	2020/02/14 	MMA 	Oddy Test (method: 20190226_OT_1 ) 	A high tack, high coverage and fast drying synthetic elastomer adhesive; Translucent, density of 6 lb/gal, 51% VOC, 15 sec - 1 min dry time; Store at 60-80°F; Contains acetone, non-volatile components, propane, cyclohexane, petroleum distillates, and hexane; Purchased January 2020, cured for 7 days before testing 	Color: Clear 	Polymer - adhesive - glue - liquid 	 	
PC-11 Marine All Purpose High Strength Epoxy 2 oz 	Protective Coating Company 	ACE Hardware 	Temporary 	2020/02/14 	MMA 	Oddy Test (method: 20190226_OT_1 ) 	2-Part epoxy; off-white but can be tinted with universal pigment; multipurpose epoxy designed for use as an adhesive, sealer or filler; high strength; 40 min work time; 24 hr cure time; 2.5g of each part mixed until uniform and spread on BoPET film with an average thickness of 1.5 mm. Catalog Number: Item no. 1002773; purchased January 2019, cured for 17 days before testing 	Color: White 	Polymer - adhesive - glue - liquid 	 	
3MRepositionable 75CA Spray Adhesive 	3M 	McMaster-Carr 	Temporary 	2020/01/02 	MMA 	Oddy Test (method: 2019226_OT_1 ) 	Low VOC pressure sensitive aerosol spray adhesive; chemical components: Acetone, 1,1-difluoroethane, propane, cycloexane, isobutane, dimethyl glutaraldehyde; sprayed onto BoPET one layer at a time waiting at least 10 seconds between each layer and left to cure an additional 24 hours before testing 	Color: White/yellow 	Polymer - adhesive - pressure-sensitive 	 	
Sikasil neutral cure SG-500 two part structural silicone adhesive 	Sikasil 	Sikasil 	FAIL 	2020/01/02 	MMA 	Oddy Test (method: 20190226_OT_1 ) 	Two-part, high modulus, neutral-curing structural silicone adhesive; Sikasil® SG-500 is manufactured in accordance with ISO 9001/14001 quality assurance system and the responsible care program; Cures in 270 minutes (~4.5 hours); Prepared using a special extrusion gun and extruded onto BoPET 24 hours before testing 	Color: Black/grey 	Polymer - adhesive - glue - liquid 	 	
Art Resin 	Art Resin Ventures, Inc. 	Art Resin Ventures, Inc. 	FAIL 	2019/12/20 	MMA 	Oddy Test (method: 20190226_OT_1 ) 	Color: Clear 	Polymer - adhesive - glue - liquid 	 	 	
Hxtal NYL-1 2-part epoxy 	Hxtal Corp. 	Talas 	FAIL 	2019/12/20 	MMA 	Oddy Test (method: 20190226_OT_1 ) 	Color: Clear 	Polymer - adhesive - glue - liquid 	 	 	
Liquid Nails Heavy Duty Construction Adhesive, LN-903 	PPG 	Unknown 	FAIL 	2019/12/20 	MMA 	Oddy Test (method: 20190226_OT_1 ) 	Low-solvent, high-strength construction adhesive for plywood, particle board, foamboard, etc; open time: 20 minutes at room temperature; applied to BoPET and spread to about 1 mm thick with a glass microscope slide and cured for 2 days before testing 	Color: Grey 	Polymer - adhesive - glue - liquid 	 	
H2O Water-Based Contact Adhesive, WA-H2O 	Wilsonart 	Unknown 	Temporary 	2019/12/20 	MMA 	Oddy Test (method: 20190226_OT_1 ) 	Liquid adhesive; 20-30 minute dry time, open time about 60 minutes; non-flammable, low VOC and VHAP content; chemical components: benzene, tetrapropylene derivatives, sulfonated sodium salts; applied to BoPET allowed to spread with gravity to about .5 mm thick, and cured for 2 days before testing 	Color: White 	Polymer - adhesive - glue - liquid 	 	
Carpenter's Wood Glue 	Elmer's 	Unknown 	FAIL 	2019/12/20 	MMA 	Oddy Test (method: 20190226_OT_1 ) 	Liquid adhesive made for furniture repair, best for woods, particle board, and porous materials; 20-30 minute clamp time, 24 hours to full bond. Applied to BoPET and spread to about 1 mm thick with a glass microscope slide and allowed to cure for 2 days before testing 	Color: Yellow 	Polymer - adhesive - glue - liquid 	 	
Glue-All Multi-Purpose Glue 	Elmer's 	Unknown 	FAIL 	2019/12/20 	MMA 	Oddy Test (method: 20190226_OT_1 ) 	Non-toxic, quick drying liquid adhesive. Curing instructions: allow to dry overnight. Applied to BoPET and spread to about 1 mm thick with a glass microscope slide and left to cure for 2 days before testing 	Color: White 	Polymer - adhesive - glue - liquid 	 	
Heritage Gummed Paper Tape #TAD101002 	Klug Conservation 	Talas 	Temporary 	2019/12/12 	MMA 	Oddy Test (method: 20190226_OT_1 ) 	Single-sided paper tape with gumming; 2.5 cm width roll; components: potato starch, paper; Received June 2019 	Color: Natural 	Polymer - adhesive - single-sided 	 	
HeatNBond Ultrahold 	Therm-o-web 	Blick Art Materials 	FAIL 	2019/12/12 	MMA 	Oddy Test (method: 20190226_OT_1 ) 	Double-sided iron on adhesive for bonding fabrics; permanent heat activated; sample material ironed between 2 sheets of BoPET before testing, removed from BoPET before testing; Purchased April 2019 	Color: Clear 	Polymer - adhesive - glue - heat activated 	 	
Heritage Gummed Paper Tape #TAD101002 	Klug Conservation 	Talas 	Temporary 	2019/11/27 	MMA 	Oddy Test (method: 20190226_OT_1 ) 	Single-sided paper tape with gumming; 2.5 cm width roll; components: potato starch, paper; Received June 2019 	Color: Natural 	Polymer - adhesive - single-sided 	 	
Scotch ATG Gold adhesive transfer tape 908, model #B0000V4PG2C 	3M 	Amazon 	Temporary 	2019/11/20 	MMA 	Oddy Test (method: 20190226_OT_1 ) 	Labeled as "acid neutral" 3M Scotch 908 ATG Gold Tape, where the gold refers to a yellow and black-plaid removable backing. 1/4 inch x 36 yards; Adhesion to Steel: 6.6 N/cm; Purchased 2019 	Color: Clear 	Polymer - adhesive - double-sided 	 	
Hot Melt Adhesive Scotch Weld (3792 LM) 	3M 	 	Temporary 	2019/06/20 	AMNH 	Oddy Test (method: MMA 20190130_OT) 	Ethylene-Vinyl Acetate Polymer - Translucent white - Cut to weight 	AMNH test #99 	Adhesive - glue - heat activated 	Copper: OK - Silver: OK - Lead: Slight darkening 	
Ultimate Optical Mount Removable (4-0167) 	Ritrama Inc. 	ColorEdge 	Unsuitable 	2019/05/14 	AMNH 	Oddy Test (method: MMA 20190130_OT) 	Called also "Optimount; Mounting film; two acrylic adhesive layers between two polyester liners - Clear - Cut to weight and tested on Mylar 	AMNH test #60 	Adhesive - pressure sensitive 	Copper: OK - Silver: OK, sample B showed very slight red tarnish - Lead: Thick orange compacted corrosion, Fluffy white crystals 	
ColorTrans CT2200 	Mactac 	Mactac 	Temporary 	2019/07/29 	AMNH 	Oddy Test (method: MMA 20190130_OT) 	Permanent/removable mounting film; 2 mil clear polyester film coated acrylic pressure sensitive adhesive - Clear - Liner removed and cut to weight 	AMNH test #172 	Adhesive - pressure sensitive 	Copper: OK - Silver: OK (sample shows droplets from condensation) - Lead: Slight darkening 	
ColorTrans CT2500 	Mactac 	Mactac 	Temporary 	2019/07/29 	AMNH 	Oddy Test (method: MMA 20190130_OT) 	Permanent self-wetting removable mounting film; 2 mil polyester film coated acrylic pressure sentitive adhesive and clear silicone pressure sensitive adhesive - Clear - Liner removed and cut to weight 	AMNH test #173 	Adhesive - pressure sensitive 	Copper: Very slight red tarnish - Silver: OK - Lead: Darkening, Violet tarnish 	
PermaTrans PUV2100 	Mactac 	Mactac 	Unsuitable 	2019/07/29 	AMNH 	Oddy Test (method: MMA 20190130_OT) 	Thin optically clear polyester film coated on both sides with acrylic pressure sensitive adhesive - Clear - Liner removed and cut to weight 	AMNH test #174 	Adhesive - pressure sensitive 	Copper: Slight red tarnish - Silver: OK - Lead: Thick orange compacted corrosion, Light white compacted corrosion 	
IMAGin Bfree Clear (JT5999MBF) 	Mactac 	Mactac 	Unsuitable 	2019/07/29 	AMNH 	Oddy Test (method: MMA 20190130_OT) 	3.1 mil gloss clear polymeric PVC film; coated on one side with a clear acrylic pressure sensitive adhesive - Transparent - Liner removed and cut to weight 	AMNH test #177 	Adhesive - pressure sensitive 	Copper: Slight red tarnish - Silver: OK - Lead: Violet tarnish (pinkish tone), Thick orange compacted corrosion, Light white compacted corrosion 	
3M VHB tape 4910 	3M 	 	Temporary 	2019/08/23 	AMNH 	Oddy Test (method: MMA 20190130_OT) 	Double-sided tape; acrylic foam - Clear - Sample was aired up for 2.5 weeks and tested on Mylar 	AMNH test #199 	Adhesive - tape - double sided 	Copper: OK - Silver: OK - Lead: Darkening, Thin Yellow/green compacted corrosion 	
3M Repositionable Tape 9415PC 	3M 	 	Temporary 	2019/09/26 	AMNH 	Oddy Test (method: MMA 20190130_OT) 	Double coated tape; acrylic adhesive - Transparent - Liner removed; cut to weight and tested on Mylar 	AMNH test #219 	Adhesive - tape - double sided 	Copper: OK - Silver: OK - Lead: A: Very slight darkening, B: Light white compacted corrosion 	
3M Repositionable Tape 9425 	3M 	 	Temporary 	2019/09/26 	AMNH 	Oddy Test (method: MMA 20190130_OT) 	Double coated tape; acrylic adhesive - Transparent - Liner removed; cut to weight and tested on Mylar 	AMNH test #220 	Adhesive - tape - double sided 	Copper: Red tarnish on sample A, sample B is OK - Silver: Blue/blue-green tarnish - Lead: Slight darkening 	
3M Double Coated Tape 415 	3M 	 	Temporary 	2019/10/15 	AMNH 	Oddy Test (method: MMA 20190130_OT) 	Acrylate copolymer adhesive; PET carrier - Transparent - Liner removed; cut to weight and tested on Mylar 	AMNH test #237 	Adhesive - tape - double sided 	Copper: OK - Silver: OK - Lead: Very slight darkening, Thin Yellow/green compacted corrosion 	
88250 Transfer Tape 	Tesa 	Tesa 	FAIL 	2019/10/24 	MMA 	Oddy Test (method: 20190226_OT_1 ) 	Water-based acrylic adhesive; 127 µm thick; no carrier, just adhesive; liner is white with blue logo; temperature resistance from -40 deg F; adhesion to steel: 64.51 N/cm; purchased November 2018 	Colorless 	Polymer - adhesive - pressure-sensitive 	 	
Photo Tex EX, adhesive printable fabric 	Lex Jet 	Lex Jet 	FAIL 	2019/10/24 	MMA 	Oddy Test (method: 20190226_OT_1 ) 	Extra strength, high tack adhesive backed printable fabric for labels, matte finish, use with solvent, latex, UV curable or eco-solvent ink; purchased August 2019 	White 	Polymer - adhesive - single-sided 	 	
Heritage Gummed Paper Tape #TAD101002 	Klug Conservation 	TALAS 	Temporary 	2019/10/23 	MMA 	Oddy Test (method: 20190226_OT_1 ) 	Single-sided paper tape with gumming; 2.5 cm width roll; components: potato starch, paper; purchased June 2019 	White 	Polymer - adhesive - single-sided 	 	
MetaScape Frost M4A-OF, adhesive vinyl 	Metamark 	RDH Supply 	FAIL 	2019/10/23 	MMA 	Oddy Test (method: 20190226_OT_1 ) 	Printable clear matte calendered PVC vinyl label with clear solvent acrylic adhesive and kraft paper lining with PE coating; frost etch 85% light transmission; 1 year shelf life, durable 3 years in vertical exposure; hazardous decomposition: carbon monoxide, carbon dioxide, hydrogen chloride, plasticizers, smoke; purchased August 2019 	Colorless 	Polymer - adhesive - single-sided 	 	
Metascape Crystal M7A-CR, adhesive vinyl 	Metamark 	RDH Supply 	FAIL 	2019/10/23 	MMA 	Oddy Test (method: 20190226_OT_1 ) 	Printable clear matte calendered PVC with clear solvent acrylic adhesive and kraft paper lining with PE coating; crystal etch 57% light transmission; 1 year shelf life, 7 year durability in vertical exposure; hazardous decomposition: carbon monoxide, carbon dioxide, hydrogen chloride, plasticizers, smoke; purchased August 2019 	Colorless 	Polymer - adhesive - single-sided 	 	
415 Double Coated Tape 	3M 	Fastenal 	Temporary 	2019/10/17 	MMA 	Oddy Test (method: 20190226_OT_1 ) 	Double sided polyester tape with 3M™ Acrylic Adhesive 400 mounted on a 60. lb densified kraft paper liner; 4.0 mil thick; 3/4 inch wide. Lot # 18169 Sub 2# 007. In the lot # the first 2 digits refer to the year of production, and the next three represent the Julian date, so date of manufacture is June 18, 2018. The tape has a 2 year shelf life from the date of manufacture when stored at 72 degrees F and 50% relative humidity; adhesion to steel: 17.65N/cm; purchased September 2019 	Colorless 	Polymer - adhesive - double-sided 	 	
Tape for Silicone Parchment Release Paper 	Unknown 	Masterpak 	Temporary 	2019/10/17 	MMA 	Oddy Test (method: 20190226_OT_1 ) 	Green tape designed to provide firm adhesion to silicone parchment release paper; catalog number: 1-913; 3.4 mil thick; purchased July 2019 	Green 	Polymer - adhesive - single-sided 	 	
Singer Heavy Duty Iron-On Fusing Web 	Shanghai Tianyang Hot Melt Adhesives Co., ltd 	Dyno LLC 	FAIL 	2019/10/17 	MMA 	Oddy Test (method: 20190226_OT_1 ) 	Iron-on fusing web; catalog number SKU: D00222; copolyamide hot melt adhesive; used in constructing storage boxes; ironed between BoPET mylar-like film according to package instructions before testing; purchased 2019 	White 	Polymer - adhesive - glue - heat activated 	 	
MACmark 8300, 832900P adhesive vinyl 	Mactac 	Mactac US 	FAIL 	2019/10/11 	MMA 	Oddy Test (method: 20190226_OT_1 ) 	Vinyl label, calendered soft vinyl (PVC) film coated with permanent acrylic adhesive on white kraft paper liner with silicone coating; 70 µm thick, durable up to 5 years, 2 year shelf life; for printed or cut labels; purchaced September 2019 	Gloss White 	Polymer - adhesive - single-sided 	 	
Heritage Gummed Paper Tape, #TAD101002 	Klug Conservation 	TALAS 	Temporary 	2019/09/24 	MMA 	Oddy Test (method: 20190226_OT_1 ) 	Single-sided paper tape with gumming; 2.5 cm width roll; components: potato starch, paper; purchased June 2019 	White 	Polymer - adhesive - single-sided 	 	
Hot Melt Adhesive 3764Q 	3M 	McMaster-Carr 	FAIL 	2019/09/24 	MMA 	Oddy Test (method: 20190226_OT_1 ) 	Low temp hot-melt glue for 3M EC and TC guns;catalog number 7333A37; ethylene-vinyl acetate polymer, naphtha, hydrocarbon resin; solid stick 5/8" x 8"; Prepared on 7/2/2019 and 7/5/2019; Extruded with a used 3M Plygun LT with Quadrack Converter. Remains of previous glue stick and first new glue stick extruded and discarded. Extruded in dots onto aluminum foil. Dots mixed in large glass lab beaker by hand wearing nitrile gloves. Purchased May 2019 	White 	Polymer - adhesive - glue - heat activated 	 	
Hot Melt Adhesive 3762Q 	3M 	McMaster-Carr 	FAIL 	2019/09/24 	MMA 	Oddy Test (method: 20190226_OT_1 ) 	Low temp hot-melt glue for 3M EC and TC Guns; catalog number 7333A35; Ethylene-Vinyl Acetate polymer, hydrocarbon resin; solid stick 5/8" x 8"; Prepared on 6/28/2019; Extruded with a used 3M Polygun LT with Quadrack Converter. Remains of previous glue stick and first new glue stick extruded and discarded. Extruded in dots onto aluminum foil. Dots mixed in large glass lab beaker by hand wearing nitrile gloves. Purchased May 2019 	Beige 	Polymer - adhesive - glue - heat activated 	 	
Dowsil 3145 Silicone Adhesive Clear MIL-A-46146, 4812MKTW 	Dow Corning 	Ellsworth Adhesive, Inc 	Temporary 	2019/09/24 	MMA 	Oddy Test (method: 20190226_OT_1 ) 	Neutral cure silicone adhesive; 90mL tube; date of manufacture: March 1, 2019 - Lot No. H050J31072; Prepared on 6/24/2019, extruded through the 1/2" nozzle opening in lines onto aluminum foil. After setting, cut into ~1cm lengths. Pieces mixed on aluminum foil by hand (wearing nitrile gloves). Purchased May 2019 	Clear 	Polymer - adhesive - glue - liquid 	 	
White A6002, adhesive vinyl 	Avery 	Avery 	FAIL 	2019/09/06 	MMA 	Oddy Test (method: 20190226_OT_1 ) 	Calendered opaque vinyl label with permanent solvent adhesive; white; purchased in 2018 	Color: White; Comment: Lead coupons in the control jars had significant blue tarnish 	Polymer - adhesive - single-sided 	 	
Vector ProV-5 Warm Red UNP, adhesive vinyl 	Beacon Graphics 	Beacon Graphics 	Temporary 	2019/09/06 	MMA 	Oddy Test (method: 20190226_OT_1 ) 	Vinyl label, soft PVC film, polyacrylate; 3 mil thick; warm red; item code: PV5391250; purchased 2018 	Color: Red, warm; Comment: Lead coupons in the control jars had significant blue tarnish 	Polymer - adhesive - single-sided 	 	
Oracal 651-091 Gold, adhesive vinyl 	Orafol 	Orafol 	Temporary 	2019/09/06 	MMA 	Oddy Test (method: 20190226_OT_1 ) 	Vinyl label, special PVC film, solvent polyacrylate, permanent, 2 year shelf life, durable up to 6 years; adhesion to steel: 46.32 N/cm; 2.5 mil thick; gold; purchased 2018 	Color: Gold; Comment: Lead coupons in the control jars had significant blue tarnish 	Polymer - adhesive - single-sided 	 	
Fastbond 30-NF Neutral Adhesive 	3M 	Pilots HQ 	Temporary 	2019/09/06 	MMA 	Oddy Test (method: 20190226_OT_1 ) 	Liquid adhesive; water-dispersed, sprayable contact adhesive for high immediate bond strength and long bonding range; bonds most foamed plastics, plastic laminate, wood, plywood, and canvas to themselves and each other; poured onto BoPET film 2 days prior to testing and allowed to spread with gravity, average thickness of 1mm; Catalog Number: 021200-21180; purchased January 2019 	Color: Tan, wood; Comment: Lead coupons in the control jars had significant blue tarnish 	Polymer - adhesive - glue - liquid 	 	
Gorilla Glue Clear 	The Gorilla Glue Company 	Gorilla Glue 	FAIL 	2019/09/06 	MMA 	Oddy Test (method: 20190226_OT_1 ) 	Multi-purpose clear liquid adhesive; dries clear and colorless; 3.75 oz bottle; full cure in 24 hours but laid out 2 days prior to testing on BoPET film. 5 six-inch long lines of glue were layed in rows about half an inch apart and smoothed together with a spatula to form an even layer of adhesive, average thickness of 0.5 mm. Purchased January 2019 	Color: Colorless, transparent; Comment: Lead coupons in the control jars had significant blue tarnish 	Polymer - adhesive - glue - liquid 	 	
OCA 8146-6 Optically Clear Adhesive 	3M 	3M 	FAIL 	2019/08/21 	MMA 	Oddy Test (method: 20190226_OT_1 ) 	Acrylic adhesive, no liner; great for bonding PMMA, glass, PET and other high surface energy and some lower surface energy substrates; adhesion to glass 6.6N/cm; received July 2019 	Colorless; Lead coupons in the control jars had significant blue tarnish 	Polymer - adhesive - pressure-sensitive 	 	
CEF 2910 Contrast Enhancement Film 	3M 	3M 	FAIL 	2019/08/21 	MMA 	Oddy Test (method: 20190226_OT_1 ) 	Pressure sensitive acrylic adhesive film, no liner; adhesion to glass 16.6N/cm; received July 2019 	Colorless; Comment: Lead coupons in the control jars had significant blue tarnish 	Polymer - adhesive - pressure-sensitive 	 	
Avery Black A6080, adhesive vinyl 	Avery 	Unknown 	Temporary 	2019/08/16 	MMA 	Oddy Test (method: 20190226_OT_1 ) 	Calendered opaque vinyl label (PVC) with permanent solvent adhesive; purchased in 2018 	Grey, Dark 	Polymer - adhesive - single-sided 	 	
530 Utility-Grade Flatback Packaging Tape 	Intertape Polymer Group 	Amazon 	FAIL 	2019/08/16 	MMA 	Oddy Test (method: 20190226_OT_1 ) 	Intertape™ brand Flatback Tape (pressure-sensitive paper tape, kraft paper tape) is designed for superior performance in a variety of packaging, splicing and tabbing applications. 2 in x 60 yds; Adhesion: 60 oz per inch; Adhesive: natural / synthetic rubber; Thickness: 7.2 mils (carrier, adhesive) 	Brown 	Polymer - adhesive - single-sided 	 	
Black Artist Tape 5326-1 	ProArt 	Amazon 	FAIL 	2019/08/16 	MMA 	Oddy Test (method: 20190226_OT_1 ) 	Black artist tape, 1 in x 60 yds; Non-glare paper tape 	Black 	Polymer - adhesive - single-sided 	 	
Acryloid B-72, SY7-05 	Unknown 	Conservation Resources 	Temporary 	2019/07/17 	MMA 	Oddy Test (method: 20190226_OT_1 ) 	B-72; tested as pellets; Chemical Components: an ethyl methacrylate co-polymer; unknown purchase date. 	Colorless, transparent 	Polymer - block/bulk/pellet 	 	
Paper tape with gumming 067-60/0; Temporary Talas part number #TAD607001 - Sold as Heritage Gummed Paper Tape #TAD101002 	Klug Conservation 	TALAS 	Temporary 	2019/07/17 	MMA 	Oddy Test (method: 20190226_OT_1 ) 	Single-sided paper tape with gumming; 2.5 cm width roll; components: potato starch, paper; purchased August 2018 	White 	Polymer - adhesive - single-sided 	 	
Frame Sealing Tape, TAD055001 	Unknown 	Talas 	PASS 	2019/07/05 	MMA 	Oddy Test (method: 20190226_OT ) 	Frame sealing tape, used as a means of sealing backing boards to frames; blue-grey pressure-sensitive tape composed of a layer of acid-free label stock, foil barrier, adhered with a non-yellowing, permanent acrylic adhesive. 	Blue-Grey 	Polymer - adhesive - single-sided 	 	
88250 Transfer Tape 	Tesa 	Tesa 	Temporary 	2018/12/19 	MMA 	Oddy Test (method: 20180821_OT ) 	Pressure-sensitive adhesive transfer tape; thickness: 127 um / 4.00 mils; colorless; no carrier just adhesive; liner is white with blue logo; temp. resistance from -40 deg F; adhesion to steel is 10 N/cm; Chemical Components: water-based acrylic adhesive; liner is polycoated paper 	Colorless 	Polymer - adhesive - pressure-sensitive 	 	
Elastosil RT480+ Catalyst T40 	Wacker 	Unknown 	FAIL 	2018/05/31 	MMA 	Oddy Test (method: 20171116_OT ) 	Arrived cured in a metal channel. Wacker Primer G790 was used to prime the channel prior to adding sealant. Received April 2018 	Natural (kind of beige) 	Polymer - adhesive - caulk or sealant 	 	
Paper tape with potato starch, #067-25/0 	Klug Conservation 	Klug Conservation 	Temporary 	2019/02/08 	AMNH 	Oddy Test (method: MMA 20190130_OT) 	Strip of paper tape with potato starch gumming - White - Cut to weight 	AMNH Test #20 	Polymer - adhesive tape - single sided 	Copper: very slight red tarnish - Silver: light purple tarnish - Lead: Darkening 	
VHB Tape 5925 double-sided 	3M 	 	Temporary 	2019/03/25 	AMNH 	Oddy Test (method: MMA 20190130_OT) 	Double coated pressure-sensitive closed-cell acrylic foam tape with modified acrylic adhesive and a PE film liner - White - Strip was cut to weight with liner removed. Tape was tested on a mylar sheet to prevent its sticking to inside of jar. 	AMNH Test #23 	Polymer - adhesive tape - double sided 	Copper: Very Slight Red Tarnish - Silver: ok - Lead: darkening, light white haze, yellow/green compacted, violet tarnish 	
Titebond II Premium Wood Glue 	Franklin International 	 	Unsuitable 	2019/03/25 	AMNH 	Oddy Test (method: MMA 20190130_OT) 	Industrial use cross-linking PVA wood glue, poured onto glass panel and allowed to dry. - Orange - Sample was scraped from panel using a razor blade. 	AMNH Test #24 	Polymer - adhesive - glue - liquid 	Copper: Spots of heavy green corrosion, heavy haze overall - Silver: yellow tarnish, black tarnish - Lead: complete corrosion, turned to powder 	
DOWSIL 791 Weatherproofing Sealant 	Dow Corning 	 	Temporary 	2019/02/08 	AMNH 	Oddy Test (method: MMA 20190130_OT) 	neutral-cure, one-part sealant; applied to Mylar and allowed to cure - Grey - Peeled/scraped from mylar 	AMNH Test #6 	Polymer - adhesive caulk 	Copper: ok - Silver: ok - Lead: darkening and thin compact corrosion (B); darkening with spots of compact corrosion (A) 	
DOWSIL 791 Weatherproofing Sealant 	Dow Corning 	 	Temporary 	2019/02/08 	AMNH 	Oddy Test (method: MMA 20190130_OT) 	neutral-cure, one-part sealant; applied to Mylar and allowed to cure - Black - Peeled/scraped from mylar 	AMNH Test #7 	Polymer - adhesive caulk 	Copper: ok - Silver: ok - Lead: darkening 	
933 Structural Glazing Sealant 	Dow Corning 	 	Unsuitable 	2019/02/08 	AMNH 	Oddy Test (method: MMA 20190130_OT) 	two-component, neutral curing silicone; applied to Mylar and allowed to cure - Black - Peeled/scraped from mylar 	AMNH Test #8 	Polymer - adhesive caulk 	Copper: Heavy haze (black); purple tarnish - Silver: ok - Lead: darkening with grey compact corrosion 	
SEA-210, GE5070 RTV Silicone Rubber compound 	GE Silicones 	 	Temporary 	2019/02/08 	AMNH 	Oddy Test (method: MMA 20190130_OT) 	Two-part silicone rubber adhesive; Applied to Mylar and allowed to cure - Grey - Peeled/scraped from mylar 	AMNH Test #9 	Polymer - adhesive caulk 	Copper: OK - Silver: OK - Lead: thin orange compact corrosion and darkening 	
Paper tape with gumming 067-60/0; Temporary Talas part number #TAD607001 - Sold as Heritage Gummed Paper Tape #TAD101002 	Klug Conservation 	TALAS 	Temporary 	2019/05/29 	MMA 	Oddy Test (method: 20190226_OT ) 	Single-sided paper tape with gumming; 2.5 cm width roll; components: potato starch, paper; purchased August 2018 	white 	Polymer - adhesive - single-sided 	 	
Synthetic Felt 	Unknown 	McMaster-Carr 	Temporary 	2019/05/29 	MMA 	Oddy Test (method: 20190226_OT ), SPME, GCMS 	1" Thick; 1/8"wide; density, lbs./sq. yd. 1.88. Material, Polyester. Hardness, Durometer 35A, Hardness Rating, Firm. Pressure to Compress 10%, psi 21. Temperature range, °F -40° to 300°. Adhesive type, rubber. Adhesive Temperature Range, °F 0° to 180°. Lengths, ft 10, 25, 50. 	white 	Polymer - adhesive - single-sided 	 	
Shurtape FP-227 high adhesion flatback paper tap. 	Shurtape 	Shurtape 	FAIL 	2019/05/29 	MMA 	Oddy Test (method: 20190226_OT ), SPME, GCMS 	Backing: Colored flatback paper. Adhesive: Rubber-based adhesive. Liner: NA. Size: 2 in. x 60 yds. Adhesion to Stainless Steel: 57 oz/in width (6.24 N/10 mm). Elongation: 2.50%. Service Temperature Range: 40 F to 150 F (4 C to 66 C). Tensile: 30 lbs/in width (52.5 N/10 mm). Thickness: 5.8 mils (0.15 mm). Purchased in Spring 2019. 	white 	Polymer - adhesive - single-sided 	 	
3M 9576, 021200-84266 Acrylic double-sided tape 	3M 	R. S. Hughes 	FAIL 	2019/05/23 	MMA 	Oddy Test (method: 20190226_OT ) 	Acrylic double-sided tape; adhesion strength 21.28 N/cm.; colorless; liner is densified kraft paper; thickness 4 mil; width 1 in; Chemical Components: carrier polypropylene; acrylic adhesive; purchased November 2018. 	colorless tape, brown liner 	Polymer - adhesive - double-sided 	 	
Fillet Tape Double Sided - 6mm x 50m, UKPFS605 	Unknown 	UK Picture Framing Supplies 	FAIL 	2019/05/23 	MMA 	Oddy Test (method: 20190226_OT ) 	Acid free double-sided acrylic tape; width 6mm; Chemical Components: acrylic adhesive; polyester carrier; purchased november 2018; repeat of Oddy 2360 and 2444. 	COLORLESS 	Polymer - adhesive - double-sided 	 	
Filmoplast SH Gummed 'linen' Tape 	Neschen 	Gaylord Archival 	FAIL 	2019/03/26 	MMA 	Oddy Test (method: 20190226_OT ), SPME, GCMS 	Neschen filmoplast SH Gummed 'Linen'Tape 50 yds.; Catalog Number: AFGLT50; Purchased: December 2018 	white 	Polymer - adhesive - single-sided 	 	
Jade 403 PVA Adhesive 	Unknown 	TALAS 	FAIL 	2019/03/14 	MMA 	Oddy Test (method: 20190214_OT_a ) 	PVA adhesive; dries transparent and colorless; Adhesive is water soluble when wet, and permanent when dry. pH neutral, acid free; modified polyvinyl acetate resin emulsion; SKU: TAD007001; Purchased: January 2019 	colorless, clear 	Polymer - adhesive - glue - liquid 	 	
PC-7 Multi-Purpose Super Strength Epoxy 2 oz. 	Protective Coating Company 	ACE hardware 	FAIL 	2019/03/14 	MMA 	Oddy Test (method: 20190214_OT_b ) 	2-Part epoxy; black; mix 1:1; 1 hr work time; mixed 3 days prior to testing; Use as adhesive, sealant, or filler; Purchased Jan 2019. 	black 	Polymer - adhesive - glue - liquid 	 	
Magic Smooth 	Wesco Enterprises 	ArtPlace 	FAIL 	2019/03/14 	MMA 	Oddy Test (method: 20190214_OT_a ), SPME GCMS	2-Part epoxy; doesn't dissolve foams; mixed 3 days prior to testing; Purchased: January 2019 	yellow 	Polymer - adhesive - glue - liquid 	 	
J-B Weld TWIN TUBE 	J-B Weld 	J-B Weld 	FAIL 	2019/03/14 	MMA 	Oddy Test (method: 20190214_OT_b ), SPME GCMS	2-Part epoxy; black; mixed 1:1; "set time 4-6 hrs; cure time 15-24 hrs" but mixed 3 days prior to testing; strength 3960 PSI; Purchased: January 2019 	black 	Polymer - adhesive - glue - liquid 	 	
Foam Fast 74 spray adhesive 	3M 	Grainger 	FAIL 	2019/03/14 	MMA 	Oddy Test (method: 20190214_OT_b ) 	Spray adhesive; aerosol can; "dries in 15 minutes" but sprayed out 2 days prior to testing; can was shaken for 2 minutes and adhesive was sprayed 3-5 inches from the surface; for bonding foam and fabric; Model/Catalog Number: Item # 3MA18; Month/Year Purchased: January 2019 	orange 	Polymer - adhesive - glue - liquid 	 	
Araldite AV 1253 + Hardener HV 1253 	Huntsman 	Conservation Resources International LLC 	FAIL 	2019/02/27 	MMA 	Oddy Test (method: 20180821_OT ) 	2-Part bulked epoxy; tan color; cure start on 1/9/19; Model/Catalog Number: AV1253, HV 1253; Purchased: August 2017; Chemical Components: Araldite: BISPHENOL A EPOXY RESIN, butyl 2,3-epoxypropyl ether. Hardener: Amides, from Me epoxyhydroxyoctadecanoate, tetraethylenepentamine and vegetable-oil fatty acids, Formaldehyde, oligomeric reaction products with phenol, titanium dioxide, 4,4'isopropylidenediphenol, Silicon, amorphous, 3,6,9-triazaundecamethylenediamine, 2,2'-iminodi(ethylamine), N(2-aminoethyl)piperazine-1,4-diethylamine, N,N,N'tris(2-aminoethyl)ethylenediamine, N(2-aminoethyl)N'[2-(1-piperazinyl)ethyl]ethylenediamine, Amines, polyethylenepoly-, trientine 	tan, blonde wood 	Polymer - adhesive - glue - liquid 	 	
RenPaste SV 427-2 / Ren HV 427-1 epoxy 	Huntsman 	restauro-online 	FAIL 	2019/02/27 	MMA 	Oddy Test (method: 20180821_OT ) 	2-Part bulked epoxy; brown; cure start on 1/9/19; Model/Catalog Number: 00051367; Purchased: September 2018; Chemical Components: Part 1: tetraethylenepentamine, 4,4'-isopropylidenediphenol. Part 2: 2,2'-[(1-methylethylidene)bis(4,1-phenyleneoxymethylene)]bisoxirane 	brown 	Polymer - adhesive - glue - liquid 	 	
Epoxy - Epocast 1645 FR A/B 	Huntsman 	Krayden Corporate 	FAIL 	2019/02/27 	MMA 	Oddy Test (method: 20180821_OT ) 	Ultra-Low Density Epoxy Void and Edge Filler; cure start on 1/9/19; Catalog Number: HT3573108; Purchased: March 2018 	red, mauve 	Polymer - adhesive - glue - liquid 	 	
Paper tape with gumming 067-60/0; Temporary Talas part number #TAD607001 - Sold as Heritage Gummed Paper Tape #TAD101002 	Klug Conservation 	TALAS 	Temporary 	2019/02/13 	MMA 	Oddy Test (method: 20180821_OT ) 	Sample material: single-sided paper tape with gumming; 2.5 cm width roll; components: potato starch, paper; purchased August 2018 	white 	Polymer - adhesive - single-sided 	 	
Sealant - Farbpaste EL FL black 9005 + WAcker Elastosil RT 480 + Wacker catalyst T 40 	Wacker 	unknown 	Unsuitable 	2018/07/31 	MMA 	Oddy Test (method: 20171116_OT ), SPME GCMS 	4-Part curable sealant; arrived cured in aluminum U-channel. Wacker Primer G 790 was used to prepare the channels for the sealant; Delivered April 2018. 	 	Polymer - adhesive - caulk or sealant 	 	
Carpet Adhesive: Commercialon Premium Modular Tile and LVT Adhesive 	Unknown 	J & J Flooring 	Unsuitable 	2018/08/02 	MMA 	Oddy Test (method: 20180525_OT ), SPME GCMS 	Acrylic-latex pressure sensitive carpet adhesive for PVC backed tiles. Instructions indicate that no more should be spread than can be covered in 2 hours.; Chemical Components: Acrylic-latex pressure sensitive adhesive; blue; Month/Year Purchased: 6/2018 	 	Polymer - adhesive - pressure-sensitive 	 	
Scotch® Long Lasting Storage Packaging Tape 	Scotch 	Amazon 	Temporary 	2018/09/13 	MMA 	Oddy Test (method: 20180706_C_OT ), SPME GCMS	Pressure-sensitive transparent colorless adhesive; catalogue #3650-6; Strong, secure, solvent-free acrylic adhesive; Chemical Components: Adhesive Type Acrylic; Purchased: April, 2017 	 	Polymer - adhesive - pressure-sensitive 	 	
Framer’s Tape II Clear 	Specialty Tapes 	Dick Blick 	Temporary 	2018/09/13 	MMA 	Oddy Test (method: 20180706_C_OT ), SPME GCMS	Archival-grade self-adhesive tape; transparent, colorless; catalogue # 23028-1002; Month/Year Purchased: April, 2017 	When this tape was put over laserjet printed paper, the black printer ink bled a bit. 	Polymer - adhesive - pressure-sensitive 	 	
Scotch® Scrapbooking Tape 	Scotch 	ULINE 	Unsuitable 	2018/09/13 	MMA 	Oddy Test (method: 20180706_C_OT ), SPME GCMS	Scotch tape; dimensions: 3/4 in x 400 in; catalogue # S-16634; Purchased: April, 2017 	 	Polymer - adhesive - pressure-sensitive 	 	
Uline painter’s masking tape 	 	ULINE 	Unsuitable 	2018/09/13 	MMA 	Oddy Test (method: 20180706_C_OT ), SPME GCMS	Blue masking tape; catalogue #S-13752; Purchased: April, 2017 	 	Polymer - adhesive - pressure-sensitive 	 	
Polyester Repair Material + Quality Hardener “cream hardener" 	McCausey Lumber 	McCausey Lumber 	Unsuitable 	2017/12/28 	MMA 	Oddy Test (method: 20171116_OT ), SPME GCMS 	100:2 by volume; Plastic filler & fillet material 302; cream hardener; off-gassed 24 hours prior to testing 	 	Polymer - adhesive - glue - liquid 	 	
Nusil CV-2680-12 	Nusil 	Unknown 	Temporary 	2018/07/24 	MMA 	Oddy Test (method: 20180525_OT ), SPME GCMS 	2-part film adhesive; colorless; CV = controlled volatility; for bonding or sealing silicone elastomers and some metals or plastics; incompatible with sulfur-cured organic rubbers, latex, chlorinated rubbers, some RTV silicones, and unreacted residues of some curing agents; Chemical Components: silicone, glass, oxide, “chemicals” (according to SDS); Purchased: 06/2018 	 	Polymer - adhesive - glue - liquid 	 	
Preservation Double Sided Tape 889 	3M Scotch 	Unknown 	Temporary 	2018/10/25 	MMA 	Oddy Test (method: 20180821_OT ), SPME GCMS 	permanent double-sided adhesive tape; colorless; 3/4" wide x 1296" long; acrylic adhesive; polyester backing; pH 7-8; transparent; purchased september 2018 	 	Polymer - adhesive - double-sided 	 	
4200 silicone tape (Red) 	Tesa 	Tesa 	Unsuitable 	2018/12/19 	MMA 	Oddy Test (method: 20180821_OT ), SPME GCMS 	red double-sided silicone adhesive tape; peel adhesion 5 N/cm; PET backing; Thickness excluding liner – 3.5mil; Chemical Components: silicone adhesive; PET liner; (info not on website yet); purchased November 2018 	 	Polymer - adhesive - double-sided 	 	
Food-Grade High-Temperature Silicone Rubber Sheet, 5827t21 	Unknown 	McMaster-Carr 	Temporary 	2018/12/19 	MMA 	Oddy Test (method: 20180821_OT ), SPME GCMS 	colorless silicone rubber sheet; 1/32" thickness; purchased 11/2018 	 	Polymer - adhesive - double-sided 	 	
3M 9731 	3M 	Unknown 	Temporary 	2019/01/11 	MMA 	Oddy Test (method: 20181031_OT ), SPME GCMS 	colorless double-sided tape; silicone adhesive on one side of polyester film carrier and acrylic adhesive on the other side; purchased fall 2018 	 	Polymer - adhesive - double-sided 	 	
Tesa® 51575 	Tesa® 	Tesa® 	Temporary 	2018/09/11 	MMA 	Oddy Test (method: 20180706_C_OT ), SPME GCMS	Double-sided tape with a non-woven backing and glassine liner; coated with a water-borne acrylic adhesive, translucent, 90 um thick, 12 mm wide; Chemical Components: acrylic adhesive, glassine liner; Purchased 8/2018; Adhesion to steel: 3.2 N/cm 	 	Polymer - adhesive - double-sided 	 	
Tesa® 4965 	Tesa® 	Tesa® 	Temporary 	2018/09/11 	MMA 	Oddy Test (method: 20180706_C_OT ), SPME GCMS	Transparent double-sided tape with high shear and temperature resistance with red liner; 0.2mm thick; Batch 01B0001-01; Chemical Components: PET backing with tackified acrylic adhesive; Purchased: 7/2018; Adhesion to steel: 8.4 N/cm (initial); 76.12 (after 14 days) 	 	Polymer - adhesive - double-sided 	 	
Tesa® 4985 	Tesa® 	Tesa® 	Temporary 	2018/09/11 	MMA 	Oddy Test (method: 20180706_C_OT ), SPME GCMS	Transparent transfer tape with no backing and light 'brown' glassine liner; 0.05 mm thick; Batch 703221; Chemical Components: tackified acrylic adhesive with no backing material/substrate; Purchased: 7/2018; Adhesion to steel: 11 N/cm (initial); 71.6 (after 14 days) 	 	Polymer - adhesive - double-sided 	 	
Tesa® 4959 	Tesa® 	Tesa® 	Temporary 	2018/09/11 	MMA 	Oddy Test (method: 20180706_C_OT ), SPME GCMS	Translucent double-sided mounting and splicing tape with non-woven backing material and light 'brown' glassine liner; 0.1 mm thick; Batch 60614H1.; Chemical Components: 'non-woven' backing and tackified acrylic adhesive; Purchased: 7/2018; Adhesion to steel: 8.5 N/cm (initial); 54.83 (after 14 days) 	 	Polymer - adhesive - double-sided 	 	
Gudy® 870, No. 614826464 	Neschen 	TALAS 	Temporary 	2018/09/27 	MMA 	Oddy Test (method: 20180821_OT ), SPME GCMS 	pressure sensitive adhesive; colorless, transparent; purchased 8/2018; 12 x 33' roll; Chemical Components: adhesive: waterbased polyacrylate dispersion; backing: double-side siliconised, white glassine paper; pH value: ~7; weight: 40 g/m^2; transverse strength: 500 g: > 5000 min, 1000 g: > 600 - 1500 min; adhesive strength: 10 min: >3,7 N/25mm, 24 hr: >5,2 N/25mm; temperature stability: -40 degrees F - 194 degrees F; purchase 8/2018 	 	Polymer - adhesive - pressure-sensitive 	 	
InstaBond C Adhesive 	unknown 	Quality Media and Laminating Solutions (QMLS) 	Unsuitable 	2018/09/27 	MMA 	Oddy Test (method: 20180821_OT ), SPME GCMS 	double-sided adhesive; Catalog Number: L#415170, R#7H22554807, PN#0470137, A#1-303058, I#1384C; Purchased 8/2018; PO#OCT-5-140; Details: thicknesses: liner & exposed adhesive = 1.1 mils; release liner = 5.1 mils nominal processing range: 50-120 degrees F; service temperature range: -30 - 200 degrees F; Peel adhesion: PSTC #103; backed w/ 1 mil polyester; exposed side = 40 oz./inch width; liner side = 40 oz./inch width; Statis shear: PSTC #107 modified; 500 gm/sq inch @ room temp.; exposed & liner side = 7+ days resistance: one applied to substrate, product is generally resistant to water, mild acids and alkalis and many solvents; outdoor durability: 2 years; shelf life: 1 year at 73 degrees F; Chemical Components: adhesive: acrylic solvent, pH neutral; carrier: 1 mil clear polyester	 	Polymer - adhesive - double-sided 	 	
Paper tape with gumming 067-60/0; Temporary Talas part number #TAD607001 - Sold as Heritage Gummed Paper Tape #TAD101002 	Klug Conservation 	TALAS 	Temporary 	2018/10/09 	MMA 	Oddy Test (method: 20180821_OT ), SPME GCMS 	Single-sided paper tape with gumming; 2.5 cm width roll; components: potato starch, paper; purchased August 2018 	 	Polymer - adhesive - single-sided 	 	
3M 431 Aluminum foil tape 	3M 	Grainger 	Temporary 	2018/10/09 	MMA 	Oddy Test (method: 20180821_OT ), SPME GCMS 	Aluminum foil tape; roll; tape width: 1"; length: 5 yd.; thickness: 3.10 mm; acrylic adhesive; tape tensile strength: 19 lb./in/; tape adhesive strength: 41 oz./in.; min tape performance temp: -65 degrees F; max tape performance temp: 300 degrees F; color: silver; purchased august 2018 	 	Polymer - adhesive - single-sided 	 	
Crystal Clear non-perf splicing tape 	Crystal Clear 	Cutfilm.com 	U 	2016/06/22 	MMA 	Oddy Test (method: 20160512_OT ) 	non-perf splicing tape; April 2016 	 	Polymer - adhesive - single-sided 	 	
J-Lar 	Shurtape 	 	U 	2016/06/22 	MMA 	Oddy Test (method: 20160512_OT ), SPME GCMS 	solvent-based acrylic packing tape; single-sided; Purchased April 2016 	 	Polymer - adhesive - single-sided 	 	
super 77 multipurpose spray adhesive 	3M 	unknown 	T 	2017/12/14 	MMA 	Oddy Test (method: 20171116_OT ), SPME GCMS 	 	 	Polymer - adhesive - glue - liquid 	 	
DP-1183 2-part Urethane Adhesive-Slo; 	BCC Products, Inc. 	McCausey Lumber 	P 	2017/12/28 	MMA 	Oddy Test (method: 20171116_OT ), SPME GCMS 	2-part polyurethane adhesive; part A resin and Part B pink hardener mixed in a 1:1 ratio and cured 24 hours 	 	Polymer - adhesive - glue - liquid 	 	
R-2141 adhesive caulk 	Nusil 	Nusil 	P 	2017/09/20 	MMA 	Oddy Test (method: 20170913_OT ), SPME GCMS 	2-part adhesive caulk; Silicone-base; Purchased 2017 	 	Polymer - adhesive - caulk or sealant 	 	
neoprene EPDM foam tape, 4311N 	Jacobs and Thompson 	Jacobs and Thompson 	T 	2018/07/24 	MMA 	Oddy Test (method: 20180525_OT ), SPME GCMS 	Neoprene EPDM foam tape, black, closed cell foam with acrylic adhesive on one side; Chemical Components: EPDM foam, acrylic adhesive; www.foamparts.com; Purchased: 5/2017; 	 	Polymer - gasket 	 	
Scotch-weld Epoxy adhesive DP 420 off white 	3M 	Amazon.com 	T 	2017/11/27 	MMA 	Oddy Test (method: 20171030_OT ), SPME GCMS 	2 PART adhesive, MIXED W/ 3M NOZZLE; purchased 10/17; cured for 3 days prior to testing 	 	Polymer - adhesive - glue - liquid 	 	
Scotch-weld urethane adhesive DP605NS off white 	3M 	Amazon.com 	T 	2017/11/27 	MMA 	Oddy Test (method: 20171030_OT ), SPME GCMS 	Urethane adhesive; cured for 5 days prior to testing; purchased 10/2017 	 	Polymer - adhesive - caulk or sealant 	 	
Gorilla white gorilla glue 	Gorilla Glue Company 	 	T 	2017/11/21 	MMA 	Oddy Test (method: 20171024_OT ) 	Waterproof adhesive; non-foaming; low odor; cured for 1 week prior to testing; 	 	Polymer - adhesive - glue - liquid 	 	
3M 96042 	3M 	 	T 	2017/09/13 	MMA 	Oddy Test (method: 20161215_OT ), SPME GCMS 	Double-sided silicone adhesive transfer tape with mylar core; purchased june 2017 	 	Polymer - adhesive - double-sided 	 	
Gorilla Heavy Duty Construction Adhesive 	Gorilla Glue Company 	 	T 	2017/08/09 	MMA 	Oddy Test (method: 20161215_OT ), SPME GCMS 	White construction adhesive; cured for 1 week before testing; purchased June 2017 	 	Polymer - adhesive - glue - liquid 	 	
PL Premium polyurethane construction adhesive; "PL3X" 	unknown 	Loctite 	Permanent 	2017/12/21 	MMA 	Oddy Test (method: 20171116_OT ), SPME GCMS 	polyurethane construction adhesive; this sample was cured 19 days before testing; purchased october 2017 	 	Polymer - adhesive - caulk or sealant 	 	
VHB 4910 double sided adhesive - with white liner 	3M 	 	Unsuitable 	2018/02/26 	MMA 	Oddy Test (method: 20171116_OT), SPME GCMS 	"general purpose acrylic" adhesive with foam core; purchased Januray 2018 	 	Polymer - adhesive - double-sided 	 	
3145 RTV MIL-A-46146 Clear adhesive sealant 	Dow Corning 	 	Temporary 	2018/02/21 	MMA 	Oddy Test (method: 20171116_OT), SPME GCMS 	cured 2 months; clear silicone adhesive 	 	Polymer - gasket 	 	
Scotch ATG Gold adhesive transfer tape 908, model #B0000V4PG2C 	3M 	Amazon 	Temporary 	2018/02/21 	MMA 	Oddy Test (method: 20171116_OT), SPME GCMS 	Details: labeled as "acid neutral" 3M Scotch 908 ATG Gold Tape, 'gold' refers to yellow and black-plaid removable backing. 1/4 inch x 36 yards; purchased januray 2018 	 	Polymer - adhesive - double-sided 	 	
Ardex Henry 622 Flooring Adhesive (petroleum solvents, urea, KOH, plus unnamed polymers), white-ish paste, translucent yellowish film 	Ardex 	Ardex 	Not suitable for use 	2016/05/09 	AWMM 	Oddy test 	Adhesives, consolidants 	 	Coating - floor (eg. stain, anti-wear, anti-slip) 	not tested on fully dried films given the full offgassing period. Should be re-tested on dried films given 4 weeks of offgassing. 	
Resene Aquaclear 	 	 	Suitable for permanent use 	1996/04/01 	AWMM 	Oddy test 	Adhesives, consolidants 	In vitrine or case 	Coating - paint & primer 	 	
Resene Polythane 	 	 	Suitable for permanent use 	1996/04/01 	AWMM 	Oddy test 	Adhesives, consolidants 	In vitrine or case 	Coating - paint & primer 	 	
Wattyl Estapol Speed Clear 	 	 	Suitable for permanent use 	1996/04/01 	AWMM 	Oddy test 	Adhesives, consolidants 	In vitrine or case 	Coating - paint & primer 	 	
Ameron Coatings AC-10 etch primer stain, Black 	 	 	Suitable for temporary use 	1999/02/24 	AWMM 	Oddy test 	Adhesives, consolidants 	Outside vitrine or case 	Coating - paint & primer 	Slight discolouration of the copper coupon. Suitable for permanent use if used sparingly and in selected situations. 	
Ameron Coatings AC-10 etch primer stain 	 	 	Suitable for permanent use 	1999/02/24 	AWMM 	Oddy test 	Adhesives, consolidants 	Outside vitrine or case 	Coating - paint & primer 	 	
Cabot’s crystal clear water-based Polyurethane 	Dulux 	 	Suitable for temporary use 	2003/01/12 	AWMM 	Oddy test 	Adhesives, consolidants 	Outside vitrine or case 	Coating - paint & primer 	Slight corrosion on one side of Pb coupon. Suitable for temporary use only with selected collections. 	
FireproC640-WD base fireproofing product and FireproC640-WD topcoat 	 	 	Suitable for temporary use 	1997/05/12 	AWMM 	Oddy test 	Adhesives, consolidants 	Outside vitrine or case 	Coating - protective (eg. anti-UV, -abbrasion, -tarnish) 	 	
Caprithane 	Croda Lusteroid Paints Ltd 	Croda Lusteroid Paints Ltd 	Suitable for temporary use 	1998/05/07 	AWMM 	Oddy test 	Adhesives, consolidants 	Outside vitrine or case 	Coating - protective (eg. anti-UV, abbrasion, tarnish) 	Slight corrosion on and dulling of Pb coupon – suitable for permanent use with selected collections; otherwise suitable only for temporary use. 	
Cotene 4610 polyethylene fluidised bed powder 	 	 	Suitable for permanent use 	1999/03/19 	AWMM 	Oddy test 	Adhesives, consolidants 	Outside vitrine or case 	Cotene 4610 polyethylene fluidised bed powder 	 	
FIWA, black 	Beele Engineering BV 	 	Suitable for permanent use 	2014/03/06 	AWMM 	Oddy test 	Adhesives, consolidants 	Outside vitrine or case 	Other - fire barrier 	 	
Quakehold gel, clear 	Ready America 	 	Suitable for permanent use 	2017/02/17 	AWMM 	Oddy test 	Adhesives, consolidants 	In vitrine or case 	Other - siicone gel 	 	
Bostik Super Contact Multi Purpose Brushable adhesive 	Bostik NZ Ltd 	Bostik NZ Ltd 	Suitable for permanent use 	2002/02/18 	AWMM 	Oddy test 	Adhesives, consolidants 	In vitrine or case 	Polymer - adhesive - glues - liquid (acrylics, wood glues, starches)	 	
Plastipad water based PVA adhesive 	Holdfast 	 	Not suitable for use 	2003/01/12 	AWMM 	Oddy test 	Adhesives, consolidants 	 	Polymer - adhesive - glues - liquid (acrylics, wood glues, starches)	 	
Evasol adhesive, clear 	 	 	Suitable for temporary use 	2015/07/22 	AWMM 	Oddy test 	Adhesives, consolidants 	Outside vitrine or case 	Polymer - adhesive - glues - liquid (acrylics, wood glues, starches)	Pb and Cu reacted visibly differently than control, but not really extreme. Probably ok if not in direct contact with object in a well ventilated area, for temporary use. 	
Aquence BG P195 (vinyl acetate butyl acrylate, methyl acrylate, water, plus other ingredients), white liquid, translucent film 	Glue Guru. Henkel New Zealand Limited 	Glue Guru. Henkel New Zealand Limited 	Not suitable for use 	2016/05/09 	AWMM 	Oddy test 	Adhesives, consolidants 	 	Polymer - adhesive - glues - liquid (acrylics, wood glues, starches)	not tested on fully dried films given the full offgassing period. Should be re-tested on dried films given 4 weeks of offgassing. 	
Aquence BG P195 (vinyl acetate butyl acrylate, methyl acrylate, water, plus other ingredients), dried film, transparent 	Glue Guru. Henkel New Zealand Limited 	Glue Guru. Henkel New Zealand Limited 	Suitable for temporary use 	2016/08/18 	AWMM 	Oddy test 	Adhesives, consolidants 	Outside vitrine or case 	Polymer - adhesive - glues - liquid (acrylics, wood glues, starches)	 	
Ardex Henry 622 Flooring Adhesive (petroleum solvents, urea, KOH, plus unnamed polymers), dried film, transparent 	Ardex 	Ardex 	Suitable for temporary use 	2016/08/18 	AWMM 	Oddy test 	Adhesives, consolidants 	Outside vitrine or case 	Polymer - adhesive - glues - liquid (acrylics, wood glues, starches)	 	
Acrifix, IR0192 	Evonik Performance Materials GMBh 	 	Unsuitable for use 	2017/02/17 	AWMM 	Oddy test 	Adhesives, consolidants 	 	Polymer - adhesive - glues - liquid (acrylics, wood glues, starches)	 	
3M Scotch-Weld Hot melt adhesive 3762-LM-Q, 3762-LM-PG, 3762-LM-TC, 3762-LM-B, 3762-LM-AE (3762-LM-Q, cloudy, colourless, slightly yellow)	EC Attwoods 	 	Permanent use, Suitable for	2014/05/07 	AWMM 	Oddy test 	Adhesives, consolidants 	In vitrine or case 	Polymer - adhesive - heat activated (hot melt, heat set) 	 	
3M Scotch-Weld Hot melt adhesive 3792-LM-Q, 3792-LM-PG, 3792-LM-TC, 3792-LM-B, 3792-LM-AE (3792-LM-Q, cloudy, colourless) 	EC Attwoods 	 	Permanent use, Suitable for	2014/05/07 	AWMM 	Oddy test 	Adhesives, consolidants 	In vitrine or case 	Polymer - adhesive - heat activated (hot melt, heat set) 	 	
Low melt glue, 3M Scotchweld, 3792 LMQ, clear 	3M New Zealand Ltd. 	3M New Zealand Ltd. 	Permanent use, Suitable for	2015/07/22 	AWMM 	Oddy test 	Adhesives, consolidants 	In vitrine or case 	Polymer - adhesive - heat activated (hot melt, heat set) 	Pretty much the same as the control. 	
3M Silicone/Acrylic Double Coated Film Tape 9731 	 	 	Permanent use, Suitable for	1998/07/20 	AWMM 	Oddy test 	Adhesives, consolidants 	Outside vitrine or case 	Polymer - adhesive tape - double sided 	 	
3M tape double sided 415 	3M 	 	Permanent use, Suitable for	2003/02/18 	AWMM 	Oddy test 	Adhesives, consolidants 	In vitrine or case 	Polymer - adhesive tape - double sided 	 	
3M Tape, Double Coated Vinyl Foam Tape, Adhesive 430, 4432, black 	3M New Zealand Ltd. 	3M New Zealand Ltd. 	Not suitable for use 	2008/02/28 	AWMM 	Oddy test 	Tapes (adhesive plus backing material) 	 	Polymer - adhesive tape - double sided 	 	
Sellotape 1205 double sided vinyl tape, colourless 	the Sellotape company 	 	Not suitable for use 	2014/05/07 	AWMM 	Oddy test 	Tapes (adhesive plus backing material) 	 	Polymer - adhesive tape - double sided 	Double sided tape used between two barrier materials does not have a large surface area exposed to offgassing, so it can still be used in appropriate circumstances. 	
3M Double sidedcoated vinyl foam tape, Tape 4432 	 	 	Not suitable for use 	2014/05/07 	AWMM 	Oddy test 	Tapes (adhesive plus backing material) 	 	Polymer - adhesive tape - double sided 	 	
Sellotape 3950 	 	 	Not suitable for use 	2003/09/16 	AWMM 	Oddy test 	Tapes (adhesive plus backing material) 	 	Polymer - adhesive tape - single sided 	 	
Sellotape 3824 	 	 	Not suitable for use 	2003/09/16 	AWMM 	Oddy test 	Tapes (adhesive plus backing material) 	 	Polymer - adhesive tape - single sided 	Moderate corrosion on all coupons. 	
Sellotape 3829 	 	 	Not suitable for use 	2003/09/16 	AWMM 	Oddy test 	Tapes (adhesive plus backing material) 	 	Polymer - adhesive tape - single sided 	 	
Gaska Tape V1515, Black 	Gaska 	 	Suitable for temporary use 	2007/11/29 	AWMM 	Oddy test 	Tapes (adhesive plus backing material) 	Outside vitrine or case 	Polymer - adhesive tape - single sided 	 	
Dual Adhesive Tape, Clear 	Frank Europe GmbH 	 	Suitable for temporary use 	2007/11/29 	AWMM 	Oddy test 	Adhesives, consolidants 	In vitrine or case 	Polymer - adhesive tape - single sided 	 	
3M VHB Tape, 4910 Tape, Clear 	3M New Zealand Ltd 	3M New Zealand Ltd. 	Suitable for permanent use 	2008/02/28 	AWMM 	Oddy test 	Adhesives, consolidants 	In vitrine or case 	Polymer - adhesive tape - single sided 	 	
VHB tape, 3M, GA14, GA14A, GA14B, clear 	Glasscorp 	Glasscorp 	Suitable for permanent use 	2015/07/22 	AWMM 	Oddy test 	Adhesives, consolidants 	In vitrine or case 	Polymer - adhesive tape - single sided 	Pretty much the same as the control. 	
Netherfield sealant for glass panels/showcases, extruded silicone, Seal M/S -004 	Netherfield Limited 	 	Suitable for temporary use 	2008/02/28 	AWMM 	Oddy test 	Adhesives, consolidants 	In vitrine or case 	Polymer - gasket 	Small specks of corrosion products on lower edge of lead coupon with uneven patina. Suitable for permanent use to apply to leading edges of doors and opposing edges. 	
S40 (previous SH4CLARL) Window Film, 3M 	 	 	Not suitable for use 	2008/02/28 	AWMM 	Oddy test 	Adhesives, consolidants 	 	Polymer - membrane (<1mm thick) 	Severe corrosion of lead coupon, loss of polish/corrosion of copper coupon, slight tarnishing of silver. Needs to be retested to establish if adhesive causes corrosion and if plastic film is permeable or would block chemical evaporating from adhesive.	
Filmoplast P90 	Neschen 	unknown 	P 	2013 	Hodgkins et. al.	Oddy Test, silver nanofilm 	acrylic adhesive on white paper carrier 	none 	TAPE 	none 	
Filmoplast P90 with Liquitex soft body mars black 	Liquitex and Neschen 	unknown 	F 	2013 	Hodgkins et. al.	Oddy Test, silver nanofilm 	black acrylic dispersion paint on acrylic adhesive white paper carrier tape 	none 	TAPE with paint 	none 	
3M double-sided tape 	3M 	unknown 	P 	2013 	Hodgkins et. al.	Oddy Test, silver nanofilm 	none 	none 	TAPE 	none 	
305 tape 	3M USA 	3M Australia 	PASS 	1997 	NAA 	PAT 	none 	none 	tape 	n/a 	
3M 415 double-sided tape 	3M USA 	3M Australia 	PASS 	1997 	NAA 	PAT 	none 	none 	tape, double-sided 	n/a 	
3M DOUBLE SIDED ADHESIVE TAPE 	3M 	3M 	P 	2009/12/23 	BM 	Oddy Test 	ACRYLIC, CLEAR, 465 	sample prep: BETWEEN MELINEX SHEETS, test #6748 	ADHESIVE, TAPE 	none 	
3M DOUBLE SIDED ADHESIVE TAPE 	3M 	3M 	T 	2009/12/23 	BM 	Oddy Test 	ARCYLIC, CLEAR, 468 MP 	sample prep: BETWEEN MELINEX SHEETS, test #6747 	ADHESIVE, TAPE 	none 	
3M SCOTCH PHOTO SPLITS 	3M 	3M 	F 	2010/04/09 	BM 	Oddy Test 	ACRYLIC ON PAPER, WHITE, 009 	sample prep: N/A, test #6791 	ADHESIVE, FILM 	none 	
3M SUPER 77 	3M 	3M 	P 	2012/09/21 	BM 	Oddy Test 	SOLVENT BASED ADHESIVE SPRAY WITH HEXONE AND PETROLIUM, CLEAR, SUPER 77 	sample prep: 48 HOURS, test #7620 	ADHESIVE 	none 	
2500 PC Tape 	3M 	unknown 	Pass 	2006/09/17 	GCI 	Oddy Test 	none 	none 	tape 	n/a 	
Adhesive 	3M 	unknown 	Fail 	1999/10/25 	GCI 	Oddy Test 	none 	none 	adhesive 	n/a 	
Adhesive 9453 	3M 	unknown 	Fail 	1991/10/01 	GCI 	Oddy Test 	none 	none 	adhesive 	n/a 	
Adhesive 9458 	3M 	Unknown 	Fail 	1991/10/01 	GCI 	Oddy Test 	none 	none 	adhesive 	n/a 	
Adhesive 9459 	3M 	unknown 	Pass w/ reservations 	1991/10/01 	GCI 	Oddy Test 	none 	none 	adhesive 	n/a 	
Adhesive Transfer Tape 465 	3M 	unknown 	Pass 	2012/02/01 	CMA 	Oddy Test 	acrylic Pressure-sensitive tape 	none 	tape, pressure-sensitive 	none 	
ALUMINIUM FOIL TAPE 	3M 	3M 	P 	2013/09/10 	BM 	Oddy Test 	ALUMINIUM FOIL, ACRYLIC ADHESIVE, SILVER, 431 	sample prep: N/A, test #7946 	ADHESIVE, TAPE 	none 	
Correction and Coverup tape #652 	3M 	Unknown 	Fail 	1994/09/13 	GCI 	Oddy Test 	none 	none 	tape 	n/a 	
DP-100 Epoxy adhesive 	3M 	Unknown 	Pass 	1993/11/10 	GCI 	Oddy Test 	none 	none 	adhesive 	n/a 	
Fast bombed 30-NF Neutral adhesive 	3M 	Unknown 	Pass 	1996/10/28 	GCI 	Oddy Test 	none 	none 	adhesive 	n/a 	
Fastbond Construction mastic (9323) 	3M 	Unknown 	Fail 	2000/09/18 	GCI 	Oddy Test 	none 	none 	adhesive 	n/a 	
High Strength Adhesive 	3M 	unknown 	Pass 	1990/05/07 	GCI 	Oddy Test 	none 	none 	adhesive 	n/a 	
Industrial Mastic (4289-NF) 	3M 	Unknown 	Fail 	2000/09/18 	GCI 	Oddy Test 	none 	none 	adhesive 	n/a 	
Jet melt hot glue (3762-PG) 	3M 	Unknown 	Fail 	2001/02/19 	GCI 	Oddy Test 	none 	none 	adhesive, hot melt 	n/a 	
Jet melt hot glue (3792-G) 	3M 	Unknown 	Pass 	2001/02/19 	GCI 	Oddy Test 	none 	none 	adhesive, hot melt 	n/a 	
Jet-melt adhesive (3764) 	3M 	Unknown 	Fail 	1996/03/03 	GCI 	Oddy Test 	none 	none 	adhesive, hot melt 	n/a 	
Laminating Acrylic Adhesives (465) 	3M 	Unknown 	Pass 	1990/09/23 	GCI 	Oddy Test 	none 	none 	adhesive 	n/a 	
Laminating Acrylic Adhesives (467) 	3M 	Unknown 	Fail 	1989/03/09 	GCI 	Oddy Test 	none 	none 	adhesive 	n/a 	
Laminating Acrylic Adhesives (9471) 	3M 	Unknown 	Fail 	1989/03/09 	GCI 	Oddy Test 	none 	none 	adhesive 	n/a 	
Laminating strips 	3M 	Unknown 	Fail 	2005/03/22 	GCI 	Oddy Test 	none 	none 	adhesive 	n/a 	
Low Temp Hot Melt Adhesive #3762 LM 	3M 	Unknown 	Fail 	1993/10/28 	GCI 	Oddy Test 	none 	none 	adhesive, hot melt 	n/a 	
Scotch roll-on adhesive 	3M 	Unknown 	Pass 	2000/09/26 	GCI 	Oddy Test 	none 	none 	tape, double sided 	n/a 	
Scotch tape #4416 	3M 	Unknown 	Fail 	2001/01/15 	GCI 	Oddy Test 	none 	none 	tape 	n/a 	
Scotch VHB foam tape 	3M 	Unknown 	Pass 	2007/05/09 	GCI 	Oddy Test 	none 	none 	tape 	n/a 	
Scotch Weld urethane adhesive 	3M 	Unknown 	Fail 	2000/03/27 	GCI 	Oddy Test 	none 	none 	adhesive 	n/a 	
Super 74 foam fast adhesive 	3M 	Unknown 	Pass 	1992/01/20 	GCI 	Oddy Test 	none 	none 	adhesive 	n/a 	
Super 77-N spray adhesive 	3M 	Unknown 	Pass 	1992/01/20 	GCI 	Oddy Test 	none 	none 	adhesive, spray 	n/a 	
Tape with adhesive: red 	3M 	Unknown 	Pass w/ reservations 	2007/03/26 	GCI 	Oddy Test 	none 	none 	tape 	n/a 	
Urethane Adhesive DP-605NS, off-white 	3M 	unknown 	Pass 	1994/02/17 	GCI 	Oddy Test 	none 	none 	adhesive 	n/a 	
VHB acylic foam tape 4910 clear 	3M 	Unknown 	Pass 	2007/03/12 	GCI 	Oddy Test 	none 	none 	tape 	n/a 	
ALUMINIUM FOIL TAPE 	AGA 	AGA 	P 	2012/11/02 	BM 	Oddy Test 	ALUMINIUM TAPE WITH ADHESIVE, SILVER, G256 	sample prep: STUCK TO ITSELF, test #7649 	ADHESIVE, TAPE 	none 	
NO MORE NAILS DOUBLE SIDED TAPE 	AMAZON (M) 	UNIBOND (S) 	F 	2013/09/10 	BM 	Oddy Test 	, CLEAR, 781746 	sample prep: N/A, test #7968 	ADHESIVE, TAPE 	none 	
BufferMount Acid-Free Removable Dry Mount Tissue 	Bienfang 	unknown 	Pass 	2009/05/15 	CMA 	Oddy Test 	Nylon fiber matrix 	none 	adhesive backed paper 	none 	
Fusion 4000 dry mount adhesive 	Bienfang Framing Products, a Division of Elmer's products Inc. 	D&K Framing Products (USA) 	PASS 	2012 	NAA 	PAT 	none 	none 	adhesive, mounting 	n/a 	
EVACON-R CONSERVATION ADHESIVE 	CONSERVATION BY DESIGN 	UNKNOWN 	F 	2012/09/08 	BM 	Oddy Test 	ETHYLENE VINYL ACRYLATE (EVA), WHITE, 	sample prep: 48 HOURS, test #7609 	ADHESIVE 	none 	
Rhoplex N-580 	Dow Chemical Company 	Conservation Resources 	Fail 	2013/09/22 	CMA 	Oddy Test 	dried adhesive dots/ aqueous dispersion of polybutyl acrylate 	for use in lieu of sticky wax 	adhesive, pressure sensitive 	 	
'Zetta Florence double-sided tape' 	DuPont USA 	Zetta Florence 	PASS 	1997 	NAA 	PAT 	unknown 	none 	tape, double-sided 	n/a 	
Tyvek (spun bonded polyolefin) tape 	DuPont USA 	Zetta Florence 	PASS 	1997 	NAA 	PAT 	(adhesive and carrier tested separately) 	none 	Tape, Tyvek 	n/a 	
STERA DOUBLE SIDED TISSUE TAPE 	DURACO 	KENWELL CONVERTERS LTD (S) 	T 	2009/08/05 	BM 	Oddy Test 	ACRYLIC, CLEAR, 2331 	sample prep: BETWEEN MELINEX SHEETS, test #6588 	ADHESIVE, TAPE 	none 	
Supalux barcode label 	The Elna Press 	The Elna Press 	PASS 	1997 	NAA 	PAT 	polypropylene base and SP240 adhesive 	adhesive and carrier tested separately 	label, barcode 	n/a 	
Elna Press #7815 barcode label 	The Elna Press 	Zetta Florence 	PASS 	1997 	NAA 	PAT 	polyester base with #310 Hi Precision acrylic adhesive (adhesive and carrier tested separately) 	none 	label, polyester and acrylic 	n/a 	
MAMMOTH TAPE POWERFUL GRIP DOUBLESIDED TAPE 	EVERBUILD (M) 	EVERBUILD (M) 	T 	2011/08/16 	BM 	Oddy Test 	, CLEAR, 	sample prep: BETWEEN MELINEX SHEETS, test #7315 	ADHESIVE, TAPE 	none 	
ACID FREE SELF ADHESIVE LINEN HANGING TAPE 	FRAMERS EQUIPMENT.COM 	FRAMERS EQUIPMENT.COM 	T 	2012/01/20 	BM 	Oddy Test 	COTTON TAPE WITH WATER BASED ACRYLIC ADHESIVE, WHITE, SLT1 	sample prep: STUCK TO ITSELF, test #7375 	ADHESIVE, TAPE 	none 	
Gripit adhesive 	Henkel Adhesives 	Henkel Adhesives 	PASS 	2002 	NAA 	PAT 	Code 3113 	none 	adhesive 	n/a 	
SELLOTAPE, DOUBLE SIDED 	HENKEL LTD (M) 	LONDON GRAPHIC CENTRE (S) 	F 	2013/09/10 	BM 	Oddy Test 	ACRYLIC ADHESIVE?, CLEAR, 50mm 	sample prep: N/A, test #7960 	ADHESIVE, TAPE 	none 	
LE PAGE PL PREMIUM CONSTRUCTION ADHESIVE 	HENKEL CANADA CORP 	UNKNOWN 	P 	2013/04/18 	BM 	Oddy Test 	POLYURETHANE, BEIGE, 	sample prep: 48 HOURS, test #7787 	ADHESIVE 	none 	
ARALDITE RAPID 	HUNTSMAN ADVANCED MATERIALS (M) 	UNKNOWN 	T 	2013/05/03 	BM 	Oddy Test 	2 PART EPOXY , CLEAR, 	sample prep: 48 HOURS, test #7824 	ADHESIVE 	none 	
ACID FREE PAPER TAPE 	KLUG CONSERVATION 	KLUG CONSERVATION 	P 	2013/01/09 	BM 	Oddy Test 	PAPER TAPE WITH POTATO STARCH ADHESIVE, WHITE, 	sample prep: STUCK TO ITSELF, test #7676 	ADHESIVE, TAPE 	none 	
LAMACOLL DOUBLE SIDED ADHESIVE FILM 	LAHMANN 	LAHMANN 	P 	2010/06/08 	BM 	Oddy Test 	ACRYLIC, CLEAR, 115H5G02 	sample prep: BETWEEN MELINEX SHEETS, test #6842 	ADHESIVE, FILM 	none 	
NORMOUNT FOAM ADHESIVE TAPE 	LEACH GRAPHICS/ NORTON PERFORMANCE PLASTICS 	LEACH GRAPHICS/ NORTON PERFORMANCE PLASTICS 	P 	2009/12/16 	BM 	Oddy Test 	POLYURETHANE FOAM WITH ACRYLIC ADHESIVE, BLACK, V2800 	sample prep: STUCK TO ITSELF, test #6761 	ADHESIVE, TAPE 	none 	
TEPPICHBAND GEWEBE (CARPET TAPE WITH CLOTH BACKING) 	LEYLANDS SDM (S) 	LEYLANDS SDM (S) 	F 	2011/08/16 	BM 	Oddy Test 	, WHITE, ART. NO. 502107000 	sample prep: STUCK TO ITSELF, test #7317 	ADHESIVE, TAPE 	none 	
DUPLOCOLL DOUBLE SIDED ADHESIVE FILM 	LOHMANN TECHNOLOGIES 	LOHMANN TECHNOLOGIES 	T 	2013/12/12 	BM 	Oddy Test 	ACRYLIC, CLEAR, VP 20391 	sample prep: N/A, test #8080 	ADHESIVE, FILM 	none 	
Filmoplast P90 	Neschen AG 	Hughes Mouldings 	PASS 	1997 	NAA 	PAT 	none 	adhesive and carrier tested separately 	tape, repair 	n/a 	
GUDY TRANSFER ADHESIVE 	NESCHEN (M) 	UNKNOWN 	P 	2010/06/08 	BM 	Oddy Test 	POLYACRYLATE AND SILICONISED GLASSINE PAPER, CLEAR, 870 	sample prep: 48 HOURS, test #6852 	ADHESIVE, FILM 	none 	
TOFFEE TAPE 	PAL ADHESIVE PRODUCTS 	PAL ADHESIVE PRODUCTS 	P 	2013/05/30 	BM 	Oddy Test 	SYNTHETIC RUBBER RESIN, CLEAR, 	sample prep: N/A, test #7859 	ADHESIVE, TAPE 	none 	
PARALOID B72 RESTORATION ADHESIVE 	ROHM AND HAAS 	CONSERVATION BY DESIGN 	P 	2013/09/10 	BM 	Oddy Test 	SOLVENT BASED ACRYLIC ADHESIVE, CLEAR, 	sample prep: 48 HOURS, test #7970 	ADHESIVE 	none 	
CELLULOSE NITRATE 	ROHM AND HAAS 	HMG Paints (S) 	P 	2013/09/10 	BM 	Oddy Test 	CELLULOSE NITRATE, CLEAR, 	sample prep: 48 HOURS, test #7980 	ADHESIVE 	none 	
MAGIC TAPE 	SCOTCH TAPE 	3M (S) 	T 	2013/09/10 	BM 	Oddy Test 	WATER BASED ADHESIVE, CLEAR, 810 	sample prep: N/A, test #7951 	ADHESIVE, TAPE 	none 	
SCOTCH TAPE 	SCOTCH TAPE MER SERVICES 	SCOTCH TAPE MER SERVICES 	T 	2012/07/22 	BM 	Oddy Test 	PAPER AND ACRYLIC ADHESIVE, BROWN, 926 TRANSFER TAPE 	sample prep: STUCK TO ITSELF, test #7586 	ADHESIVE, TAPE 	none 	
DOUBLE SIDED FABRIC TAPE 	SEALANT AND TOOLS DIRECT 	SEALANT AND TOOLS DIRECT 	T 	2013/04/19 	BM 	Oddy Test 	, CLEAR, 4934 	sample prep: BETWEEN MELINEX SHEETS, test #7796 	ADHESIVE, TAPE 	none 	
DOUBLE SIDED PE MOUNTED TAPE 	SEALANT AND TOOLS DIRECT 	SEALANT AND TOOLS DIRECT 	T 	2013/04/19 	BM 	Oddy Test 	PE FOAM WITH ADHESIVE, CLEAR, 4952 	sample prep: BETWEEN MELINEX SHEETS, test #7800 	ADHESIVE, TAPE 	none 	
TESA DOUBLE-COATED TAPE WITH HIGH SHEAR AND TEMPERATURE RESISTANCE 	TESA 	SEALANT AND TOOLS DIRECT (S) 	P 	2012/06/06 	BM 	Oddy Test 	PET BACKING, ACRYLIC ADHESIVE, CLEAR, 4965 	sample prep: BETWEEN MELINEX SHEETS, test #7530 	ADHESIVE, TAPE 	none 	
TESA DOUBLE-SIDED FABRIC TAPE 	TESA 	SEALANT AND TOOLS DIRECT (S) 	F 	2012/06/06 	BM 	Oddy Test 	FABRIC BACKING, SYNTHETIC RUBBER ADHESIVE, CLEAR, 4934 	sample prep: BETWEEN MELINEX SHEETS, test #7526 	ADHESIVE, TAPE 	none 	
TESA DOUBLE-SIDED FILMIC HIGH ADHESION TAPE 	TESA 	SEALANT AND TOOLS DIRECT (S) 	P 	2012/06/06 	BM 	Oddy Test 	PVC FILM BACKING, ACRYLIC ADHESIVE, WHITE, 4970 	sample prep: BETWEEN MELINEX SHEETS, test #7529 	ADHESIVE, TAPE 	none 	
TESA DOUBLE-SIDED NON-WOVEN TAPE 	TESA 	SEALANT AND TOOLS DIRECT (S) 	P 	2012/06/06 	BM 	Oddy Test 	ACRYLIC ADHESIVE, CLEAR, 4959 	sample prep: BETWEEN MELINEX SHEETS, test #7534 	ADHESIVE, TAPE 	none 	
TESA DOUBLE-SIDED NON-WOVEN TAPE 	TESA 	SEALANT AND TOOLS DIRECT (S) 	P 	2012/06/06 	BM 	Oddy Test 	WATER-BASED ACRYLIC ADHESIVE, CLEAR, 51575 	sample prep: BETWEEN MELINEX SHEETS, test #7527 	ADHESIVE, TAPE 	none 	
TESA DOUBLE-SIDED PE FOAM MOUNTING TAPE 	TESA 	SEALANT AND TOOLS DIRECT (S) 	P 	2012/06/06 	BM 	Oddy Test 	PE FOAM, ACRYLIC ADHESIVE, WHITE, 4952 	sample prep: BETWEEN MELINEX SHEETS, test #7531 	ADHESIVE, TAPE 	none 	
TESA DOUBLE-SIDED PE FOAM MOUNTING TAPE 	TESA 	SEALANT AND TOOLS DIRECT (S) 	P 	2012/06/06 	BM 	Oddy Test 	PE FOAM, ACRYLIC ADHESIVE, WHITE, 4957 	sample prep: BETWEEN MELINEX SHEETS, test #7532 	ADHESIVE, TAPE 	none 	
TESA DOUBLE-SIDED PE FOAM MOUNTING TAPE 	TESA 	SEALANT AND TOOLS DIRECT (S) 	P 	2012/06/06 	BM 	Oddy Test 	PE FOAM, ACRYLIC ADHESIVE, BLACK, 62936 	sample prep: BETWEEN MELINEX SHEETS, test #7535 	ADHESIVE, TAPE 	none 	
TESA DOUBLE-SIDED TAPE WITH FABRIC BACKING 	TESA 	SEALANT AND TOOLS DIRECT (S) 	P 	2012/06/06 	BM 	Oddy Test 	CLOTH, NATURAL RUBBER ADHESIVE, WHITE, 4964 	sample prep: BETWEEN MELINEX SHEETS, test #7533 	ADHESIVE, TAPE 	none 	
TESA TACKY TRANSFER TAPE, DOUBLE SIDED 	TESA 	SEALANT AND TOOLS DIRECT (S) 	P 	2012/06/06 	BM 	Oddy Test 	MODIFIED ACRYLIC ADHESIVE, CLEAR, 4985 	sample prep: BETWEEN MELINEX SHEETS, test #7528 	ADHESIVE, TAPE 	none 	
Splicing tape 	unknown 	Christy's Editorial Film and Video supply 	PASS 	1997 	NAA 	PAT 	25 mm 	adhesive and carrier tested separately 	tape, splicing 	n/a 	
Evasol 	unknown 	Conservation Resources 	PASS 	2003 	NAA 	PAT 	EVA, buffered, acid-free and reversible 	none 	adhesive 	n/a 	
Fuji archival laminating film 	unknown 	Direct National Business Machines and Supplies	PASS 	2006 	NAA 	PAT 	none 	none 	film, laminating 	n/a 	
'Cine Care' film Splicing tape 	unknown 	John Barry 	PASS 	1997 	NAA 	PAT 	16 mm 	adhesive and carrier tested separately 	tape, splicing 	n/a 	
KLUCEL G 	UNKNOWN 	PRESERVATION EQUIPMENT LTD (S) 	P 	2013/09/10 	BM 	Oddy Test 	CELLULOSE ETHER, CLEAR, 	sample prep: 48 HOURS, test #7997 	ADHESIVE 	none 	
LASCAUX ADHESIVE 	UNKNOWN 	PRESERVATION EQUIPMENT LTD (S) 	P 	2013/09/10 	BM 	Oddy Test 	ACRYLIC EMULSION, CLEAR, D360 	sample prep: 48 HOURS, test #7989 	ADHESIVE 	none 	
LINECO NEUTRAL PH ADHESIVE 	UNKNOWN 	PRESERVATION EQUIPMENT LTD (S) 	T 	2013/09/10 	BM 	Oddy Test 	POLYVINYL ACRYLATE (PVA), CLEAR, 901-1128 	sample prep: 48 HOURS, test #7974 	ADHESIVE 	none 	
LOW MELT ADHESIVE 	UNKNOWN 	PRESERVATION EQUIPMENT LTD (S) 	T 	2012/08/14 	BM 	Oddy Test 	, WHITE, PEL 419-1044 BATCH 1117422 	sample prep: MELTED AND COOLED, test #7600 	ADHESIVE 	none 	
TYVEK ADHESIVE TAPE 	UNKNOWN 	PRESERVATION EQUIPMENT LTD (S) 	F 	2013/09/16 	BM 	Oddy Test 	POLYETHYLENE, ACRYLIC ADHESIVE, WHITE, 57MM, 804-2250 	sample prep: STUCK TO ITSELF, test #8021 	ADHESIVE, TAPE 	none 	
Nichiban Double Sided Tape 	unknown 	Regal Craft Cards 	PASS 	2012 	NAA 	PAT 	6mm 	none 	tape, double-sided 	n/a 	
Optically clear double sided mounting film 	unknown 	Starleaton Digital Solutions 	PASS 	2012 	NAA 	PAT 	none 	none 	film, mounting 	n/a 	
CARBOXY METHYL CELLULOSE 	UNKNOWN 	UNKNOWN 	P 	2013/09/10 	BM 	Oddy Test 	CARBOXY METHYL CELLULOSE, CLEAR, 	sample prep: 48 HOURS, test #8001 	ADHESIVE 	none 	
CLAM 58 	UNKNOWN 	UNKNOWN 	P 	2013/09/10 	BM 	Oddy Test 	VINYL ACRYLIC, CLEAR, 	sample prep: 48 HOURS, test #7993 	ADHESIVE 	none 	
MOWILITH 50 (50% IN IMS) 	UNKNOWN 	UNKNOWN 	P 	2013/09/10 	BM 	Oddy Test 	PVA , CLEAR, 	sample prep: 48 HOURS, test #7984 	ADHESIVE 	none 	
glazing sealant tape 	Work Site 	unknown 	Fail 	2000/03/21 	GCI 	Oddy Test 	none 	none 	tape 	n/a 	
WORLD BRAND 300 ADHESIVE 	WORLD BRAND (M) 	UNKNOWN 	P 	2013/02/25 	BM 	Oddy Test 	POLYCHLOROPRENE RUBBER, YELLOW, 300 	sample prep: 48 HOURS, test #7705 	ADHESIVE 	none 	
Economy Hot Glue 	 	 	Temporary to FAIL 	2016/7 	IMA 	Oddy Test, Microchemical Tests, and EGA 	Ethylene Vinyl Acetate Polymer 	 	ADHESIVE 	 	
Economy Hot Glue 	 	 	Temporary to FAIL 	2016/7 	IMA 	Oddy Test, Microchemical Tests, and EGA 	Isobutylene/Butane Copolymer 	 	ADHESIVE 	 	
3M Double Sided Tape 	3M 	Preservation Equipment Ltd 	FAIL 	2019/02/14 	HCC 	Oddy Test 	--- 	none 	Polymer - adhesive tape - double sided 	100px 	
Kap Bond Acid-free Repair Glue 	--- 	Promatech Singapore 	FAIL 	2019/02/14 	HCC 	Oddy Test 	--- 	none 	Polymer - adhesive sealant 	100px 	
Silicone Release Tape 	Talas 	Talas 	PASS 	2021/02/22 	NYUL 	Oddy Test 	Tape designed to adhere to silicone-coated surfaces. Catalog number SKU: TPB018001. 	Color: Green 	Polymer - adhesive tape - single sided 	100px 	
==List of Manufacturers and Suppliers==
* 3M
* 3M Australia
* Bienfang
* Christy's Editorial Film and Video Supply (USA)
* Conservation Resources
* D&K Framing Products (USA)
* Direct National Business Machines and Supplies
* Dow Chemical Co
* DuPont USA
* The Elna Press
* Henkel Adhesives (Australia/New Zealand)
* Hughes Mouldings (07) 3275 4321
* John Barry
* Liquitex
* Neschen AG (Germany)
* Neschen US
* Regal Craft Cards
* Starleaton Digital Solutions
* Work Site
* Zetta Florence
==External Links==
Category:Exhibition
Category:Testing
Choosing Materials